# Electronic Supplementary Material (ESI) for CrystEngComm.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1868911'
loop_
_audit_author_name
_audit_author_address
H[Ni0.5(en)(H2O)][Ni6(en)3(OAc)2(tris)(H2O)2(B-?-PW9O34)]"5H2O
;BIT
China
;
_audit_update_record             
;
2018-09-21 deposited with the CCDC.	2019-03-11 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C32 H126 N18 Ni13 O98 P2 W18'
_chemical_formula_weight         6465.97

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/c'
_space_group_name_Hall           '-P 2ybc'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   12.3192(3)
_cell_length_b                   22.2133(6)
_cell_length_c                   24.4657(13)
_cell_angle_alpha                90
_cell_angle_beta                 94.038(4)
_cell_angle_gamma                90
_cell_volume                     6678.4(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       ?
_exptl_crystal_colour            ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.215
_exptl_crystal_F_000             5908
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.140
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.100
_exptl_absorpt_coefficient_mu    17.340
_shelx_estimated_absorpt_T_min   0.195
_shelx_estimated_absorpt_T_max   0.276
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            36516
_diffrn_reflns_av_unetI/netI     0.1311
_diffrn_reflns_av_R_equivalents  0.1174
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_theta_min         2.875
_diffrn_reflns_theta_max         24.998
_diffrn_reflns_theta_full        24.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             11742
_reflns_number_gt                7636
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0855P)²+199.4867P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         11742
_refine_ls_number_parameters     819
_refine_ls_number_restraints     122
_refine_ls_R_factor_all          0.1400
_refine_ls_R_factor_gt           0.0862
_refine_ls_wR_factor_ref         0.2179
_refine_ls_wR_factor_gt          0.1918
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_restrained_S_all      1.059
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 0.4224(3) 0.77279(15) 0.05354(16) 0.0364(9) Uani 1 1 d . . . . .
Ni2 Ni 0.3114(3) 0.82100(13) 0.15138(15) 0.0280(8) Uani 1 1 d . . . . .
Ni3 Ni 0.5237(2) 0.74125(14) 0.17109(14) 0.0265(8) Uani 1 1 d . . . . .
Ni4 Ni 0.2277(2) 0.88088(14) 0.25681(15) 0.0300(8) Uani 1 1 d . . . . .
Ni5 Ni 0.4160(2) 0.79895(13) 0.27093(14) 0.0248(7) Uani 1 1 d . . . . .
Ni6 Ni 0.6280(2) 0.72765(15) 0.29033(16) 0.0314(8) Uani 1 1 d . . . . .
Ni7 Ni 0.000000 0.000000 0.500000 0.068(2) Uani 1 2 d S . P . .
P1 P 0.2899(4) 0.6869(2) 0.2073(2) 0.0072(10) Uani 1 1 d . U . . .
W1 W 0.41077(8) 0.61804(4) 0.09420(5) 0.0267(3) Uani 1 1 d . . . . .
W2 W 0.52385(8) 0.59315(4) 0.22461(5) 0.0260(3) Uani 1 1 d . . . . .
W3 W 0.15691(8) 0.59137(4) 0.30303(5) 0.0283(3) Uani 1 1 d . . . . .
W4 W 0.40058(8) 0.66016(5) 0.34325(5) 0.0270(3) Uani 1 1 d . . . . .
W5 W 0.16274(8) 0.71090(5) 0.07334(5) 0.0302(3) Uani 1 1 d . . . . .
W6 W 0.04906(8) 0.77446(4) 0.18420(5) 0.0284(3) Uani 1 1 d . . . . .
W7 W 0.17077(8) 0.74478(4) 0.32339(5) 0.0267(3) Uani 1 1 d . . . . .
W8 W 0.03159(8) 0.62120(5) 0.16292(5) 0.0293(3) Uani 1 1 d . . . . .
W9 W 0.27916(8) 0.52555(4) 0.18184(5) 0.0273(3) Uani 1 1 d . . . . .
C1 C 0.581(2) 0.7239(14) -0.0119(14) 0.074(6) Uani 1 1 d D U . . .
H1A H 0.595262 0.690763 0.013338 0.089 Uiso 1 1 calc R U . . .
H1B H 0.642243 0.727967 -0.034181 0.089 Uiso 1 1 calc R U . . .
C2 C 0.4791(17) 0.7100(13) -0.0486(11) 0.044(7) Uani 1 1 d D U . . .
H2A H 0.478881 0.733657 -0.081952 0.053 Uiso 1 1 calc R U . . .
H2B H 0.478061 0.667722 -0.058552 0.053 Uiso 1 1 calc R U . . .
C3 C 0.113(3) 0.9920(17) 0.2465(17) 0.073(10) Uani 1 1 d . U . . .
H3A H 0.081008 1.022780 0.222206 0.088 Uiso 1 1 calc R U . . .
H3B H 0.143339 1.011465 0.279614 0.088 Uiso 1 1 calc R U . . .
C4 C 0.030(2) 0.9488(14) 0.2598(16) 0.059(10) Uani 1 1 d . . . . .
H4A H -0.020302 0.968120 0.282992 0.070 Uiso 1 1 calc R U . . .
H4B H -0.010543 0.936341 0.226333 0.070 Uiso 1 1 calc R U . . .
C5 C 0.812(3) 0.6588(19) 0.3383(19) 0.085(13) Uani 1 1 d . . . . .
H5A H 0.847025 0.687500 0.363814 0.102 Uiso 1 1 calc R U . . .
H5B H 0.840421 0.619061 0.347424 0.102 Uiso 1 1 calc R U . . .
C6 C 0.835(3) 0.6743(15) 0.2827(15) 0.054(8) Uani 1 1 d . U . . .
H6A H 0.912883 0.677971 0.280324 0.065 Uiso 1 1 calc R U . . .
H6B H 0.808837 0.642456 0.258024 0.065 Uiso 1 1 calc R U . . .
C7 C 0.203(4) 0.074(2) 0.516(2) 0.100(13) Uani 1 1 d . U . . .
H7A H 0.247675 0.104859 0.501105 0.120 Uiso 1 1 calc R U . . .
H7B H 0.207705 0.076949 0.555552 0.120 Uiso 1 1 calc R U . . .
C8 C 0.237(3) 0.0112(16) 0.4974(18) 0.075(12) Uani 1 1 d . . . . .
H8A H 0.309586 0.001834 0.512612 0.090 Uiso 1 1 calc R U . . .
H8B H 0.235848 0.009425 0.457789 0.090 Uiso 1 1 calc R U . . .
C9 C 0.300(3) 0.8881(17) 0.0495(17) 0.075(5) Uani 1 1 d D U . . .
C10 C 0.249(3) 0.9349(16) 0.0101(16) 0.077(5) Uani 1 1 d D U . . .
H10A H 0.280738 0.973580 0.018367 0.115 Uiso 1 1 calc R U . . .
H10B H 0.171851 0.936817 0.013796 0.115 Uiso 1 1 calc R U . . .
H10C H 0.261931 0.923932 -0.026848 0.115 Uiso 1 1 calc R U . . .
C11 C 0.4060(18) 0.9028(10) 0.3430(10) 0.020(5) Uani 1 1 d . U . . .
C12 C 0.459(2) 0.9419(12) 0.3908(11) 0.032(6) Uani 1 1 d . . . . .
H12A H 0.505677 0.971646 0.376184 0.048 Uiso 1 1 calc R U . . .
H12B H 0.501458 0.916458 0.415916 0.048 Uiso 1 1 calc R U . . .
H12C H 0.403316 0.961441 0.409657 0.048 Uiso 1 1 calc R U . . .
C13 C 0.611(2) 0.8483(12) 0.2263(15) 0.053(9) Uani 1 1 d . . . . .
H13A H 0.679118 0.839956 0.209880 0.063 Uiso 1 1 calc R U . . .
H13B H 0.629458 0.868154 0.261059 0.063 Uiso 1 1 calc R U . . .
C14 C 0.533(2) 0.8664(13) 0.1320(12) 0.039(7) Uani 1 1 d . . . . .
H14A H 0.499163 0.896787 0.107885 0.047 Uiso 1 1 calc R U . . .
H14B H 0.604643 0.858205 0.119566 0.047 Uiso 1 1 calc R U . . .
C15 C 0.4409(19) 0.9117(11) 0.2083(11) 0.029(6) Uani 1 1 d . U . . .
H15A H 0.454649 0.934946 0.241638 0.034 Uiso 1 1 calc R U . . .
H15B H 0.406537 0.938248 0.180787 0.034 Uiso 1 1 calc R U . . .
C16 C 0.546(2) 0.8916(11) 0.1895(11) 0.029(6) Uani 1 1 d . U . . .
N1 N 0.567(2) 0.7796(12) 0.0190(13) 0.074(6) Uani 1 1 d D U . . .
H1C H 0.566891 0.811308 -0.003147 0.088 Uiso 1 1 calc R U . . .
H1D H 0.621131 0.783740 0.044845 0.088 Uiso 1 1 calc R U . . .
N2 N 0.3825(18) 0.7247(11) -0.0187(9) 0.046(6) Uani 1 1 d D . . . .
H2C H 0.348937 0.690768 -0.010554 0.055 Uiso 1 1 calc R U . . .
H2D H 0.336526 0.746452 -0.040369 0.055 Uiso 1 1 calc R U . . .
N3 N 0.1956(17) 0.9614(8) 0.2207(10) 0.035(6) Uani 1 1 d . . . . .
H3C H 0.255776 0.983701 0.222559 0.042 Uiso 1 1 calc R U . . .
H3D H 0.174815 0.955782 0.185476 0.042 Uiso 1 1 calc R U . . .
N4 N 0.0754(16) 0.8963(11) 0.2875(13) 0.055(8) Uani 1 1 d . . . . .
H4C H 0.032065 0.864683 0.281023 0.065 Uiso 1 1 calc R U . . .
H4D H 0.082818 0.902609 0.323494 0.065 Uiso 1 1 calc R U . . .
N5 N 0.6905(16) 0.6600(11) 0.3427(11) 0.042(6) Uani 1 1 d . . . . .
H5C H 0.675121 0.667646 0.376968 0.050 Uiso 1 1 calc R U . . .
H5D H 0.661529 0.624552 0.332769 0.050 Uiso 1 1 calc R U . . .
N6 N 0.7835(18) 0.7297(10) 0.2662(10) 0.040(6) Uani 1 1 d . . . . .
H6C H 0.782686 0.733908 0.229990 0.048 Uiso 1 1 calc R U . . .
H6D H 0.819698 0.760627 0.281807 0.048 Uiso 1 1 calc R U . . .
N7 N 0.081(3) 0.0799(13) 0.4920(13) 0.081(10) Uani 1 1 d . . . . .
H7C H 0.078906 0.090131 0.456794 0.098 Uiso 1 1 calc R U . . .
H7D H 0.047461 0.108748 0.509855 0.098 Uiso 1 1 calc R U . . .
N8 N 0.154(3) -0.0342(15) 0.5186(16) 0.090(11) Uani 1 1 d . . . . .
H8C H 0.165405 -0.038994 0.554657 0.108 Uiso 1 1 calc R U . . .
H8D H 0.160627 -0.069809 0.502557 0.108 Uiso 1 1 calc R U . . .
N9 N 0.6104(19) 0.9490(11) 0.1815(12) 0.062(9) Uani 1 1 d . . . . .
H9A H 0.582135 0.983426 0.187924 0.074 Uiso 1 1 calc R U . . .
H9B H 0.675069 0.946976 0.170417 0.074 Uiso 1 1 calc R U . . .
O1 O 0.5628(13) 0.7945(7) 0.2367(8) 0.031(4) Uani 1 1 d . . . . .
O2 O 0.4687(14) 0.8120(7) 0.1271(8) 0.033(5) Uani 1 1 d . . . . .
O3 O 0.3673(11) 0.8647(7) 0.2187(7) 0.020(4) Uani 1 1 d . . . . .
O4 O 0.4647(13) 0.8587(8) 0.3301(7) 0.030(4) Uani 1 1 d . . . . .
O5 O 0.3154(14) 0.9182(7) 0.3263(8) 0.033(4) Uani 1 1 d . . . . .
O6 O 0.4647(13) 0.6942(8) 0.1035(7) 0.029(4) Uani 1 1 d . . . . .
O7 O 0.2718(13) 0.7648(7) 0.0891(8) 0.032(4) Uani 1 1 d . . . . .
O8 O 0.5656(12) 0.6718(7) 0.2215(7) 0.030(4) Uani 1 1 d . . . . .
O9 O 0.3634(12) 0.7438(7) 0.2033(7) 0.025(4) Uani 1 1 d . U . . .
O10 O 0.1643(12) 0.8231(7) 0.1873(7) 0.024(4) Uani 1 1 d . U . . .
O11 O 0.4674(12) 0.7252(7) 0.3138(7) 0.026(4) Uani 1 1 d . . . . .
O12 O 0.2609(13) 0.7977(7) 0.2936(7) 0.027(4) Uani 1 1 d . . . . .
O13 O 0.4575(13) 0.5957(8) 0.0329(8) 0.032(4) Uani 1 1 d . . . . .
O14 O 0.2693(12) 0.6476(8) 0.0712(8) 0.033(4) Uani 1 1 d . . . . .
O15 O 0.1261(16) 0.7205(9) 0.0048(8) 0.047(5) Uani 1 1 d . . . . .
O16 O 0.0621(14) 0.7644(7) 0.1070(8) 0.032(4) Uani 1 1 d . . . . .
O17 O -0.0613(14) 0.8228(8) 0.1857(8) 0.036(4) Uani 1 1 d . U . . .
O18 O 0.0711(13) 0.7537(8) 0.2594(8) 0.033(4) Uani 1 1 d . . . . .
O19 O 0.1063(15) 0.7860(8) 0.3712(8) 0.042(5) Uani 1 1 d . . . . .
O20 O 0.2895(12) 0.7130(7) 0.3700(7) 0.026(4) Uani 1 1 d . . . . .
O21 O 0.4819(15) 0.6452(8) 0.4033(9) 0.043(5) Uani 1 1 d . . . . .
O22 O 0.4591(13) 0.6069(7) 0.2946(7) 0.028(4) Uani 1 1 d . . . . .
O23 O 0.6411(14) 0.5557(8) 0.2452(9) 0.042(5) Uani 1 1 d . . . . .
O24 O 0.5262(13) 0.5886(7) 0.1475(8) 0.035(5) Uani 1 1 d . . . . .
O25 O 0.3494(11) 0.6325(7) 0.1850(7) 0.022(4) Uani 1 1 d . . . . .
O26 O 0.1839(12) 0.6946(7) 0.1725(7) 0.028(4) Uani 1 1 d . . . . .
O27 O 0.2682(11) 0.6761(6) 0.2664(7) 0.021(4) Uani 1 1 d . . . . .
O28 O 0.3363(13) 0.5439(7) 0.1151(7) 0.029(4) Uani 1 1 d . . . . .
O29 O 0.0595(13) 0.6466(8) 0.0922(8) 0.037(5) Uani 1 1 d . . . . .
O30 O -0.0293(12) 0.6964(7) 0.1771(8) 0.031(4) Uani 1 1 d . . . . .
O31 O 0.2826(13) 0.5970(7) 0.3481(7) 0.029(4) Uani 1 1 d . U . . .
O32 O 0.1093(12) 0.6641(8) 0.3343(8) 0.033(4) Uani 1 1 d . . . . .
O33 O 0.4205(11) 0.5230(7) 0.2153(7) 0.028(4) Uani 1 1 d . . . . .
O34 O 0.1440(12) 0.5626(7) 0.1547(8) 0.033(4) Uani 1 1 d . . . . .
O35 O 0.0616(12) 0.6089(7) 0.2387(7) 0.025(4) Uani 1 1 d . U . . .
O36 O 0.2324(12) 0.5429(7) 0.2543(7) 0.023(4) Uani 1 1 d . U . . .
O37 O 0.2491(16) 0.4489(8) 0.1754(9) 0.044(5) Uani 1 1 d . . . . .
O38 O -0.0826(11) 0.5783(8) 0.1493(7) 0.029(4) Uani 1 1 d . . . . .
O39 O 0.0881(14) 0.5400(8) 0.3376(8) 0.038(5) Uani 1 1 d . . . . .
O40 O 0.371(3) 0.8530(10) 0.0202(10) 0.079(8) Uani 1 1 d . . . . .
O41 O 0.274(2) 0.8930(11) 0.1010(12) 0.075(5) Uani 1 1 d . U . . .
O1W O 0.6829(12) 0.7405(9) 0.1447(8) 0.039(5) Uani 1 1 d . . . . .
O2W O 0.6564(14) 0.7913(8) 0.3509(9) 0.043(5) Uani 1 1 d . . . . .
O3W O 0.012(3) -0.0249(14) 0.4144(13) 0.109(11) Uani 1 1 d . . . . .
O4W O 0.816(2) 0.9213(13) 0.1462(15) 0.102(10) Uani 1 1 d . . . . .
O5W O 0.7242(16) 0.6288(10) 0.1108(10) 0.059(6) Uani 1 1 d . . . . .
O6W O 0.919(2) 0.7006(18) 0.9431(13) 0.118(12) Uani 1 1 d . . . . .
O7W O 0.185(2) 0.8935(11) 0.4160(11) 0.078(8) Uani 1 1 d . . . . .
O8W O 0.142(2) 0.3405(12) 0.1589(15) 0.105(11) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ni1 N1 2.03(3) . ?
Ni1 O40 2.04(2) . ?
Ni1 O2 2.044(19) . ?
Ni1 N2 2.09(2) . ?
Ni1 O7 2.111(17) . ?
Ni1 O6 2.174(18) . ?
Ni2 O3 1.992(16) . ?
Ni2 O7 2.003(18) . ?
Ni2 O41 2.05(3) . ?
Ni2 O10 2.070(16) . ?
Ni2 O2 2.076(17) . ?
Ni2 O9 2.203(17) . ?
Ni3 O2 1.995(18) . ?
Ni3 O8 2.019(18) . ?
Ni3 O1 2.025(18) . ?
Ni3 O6 2.045(17) . ?
Ni3 O1W 2.108(15) . ?
Ni3 O9 2.178(16) . ?
Ni4 N3 2.02(2) . ?
Ni4 O3 2.045(14) . ?
Ni4 O12 2.083(16) . ?
Ni4 N4 2.10(2) . ?
Ni4 O5 2.118(19) . ?
Ni4 O10 2.228(17) . ?
Ni5 O3 2.006(16) . ?
Ni5 O4 2.023(17) . ?
Ni5 O11 2.024(16) . ?
Ni5 O12 2.026(16) . ?
Ni5 O1 2.048(17) . ?
Ni5 O9 2.124(17) . ?
Ni6 N6 2.04(2) . ?
Ni6 O2W 2.06(2) . ?
Ni6 N5 2.09(2) . ?
Ni6 O11 2.099(14) . ?
Ni6 O1 2.103(18) . ?
Ni6 O8 2.186(17) . ?
Ni7 N7 2.05(3) . ?
Ni7 N7 2.05(3) 3_556 ?
Ni7 N8 2.06(3) . ?
Ni7 N8 2.06(3) 3_556 ?
Ni7 O3W 2.18(3) . ?
Ni7 O3W 2.18(3) 3_556 ?
P1 O27 1.509(17) . ?
P1 O26 1.517(17) . ?
P1 O25 1.532(16) . ?
P1 O9 1.561(16) . ?
W1 O13 1.717(18) . ?
W1 O6 1.826(17) . ?
W1 O14 1.910(15) . ?
W1 O28 1.970(16) . ?
W1 O24 1.972(18) . ?
W1 O25 2.418(15) . ?
W2 O23 1.711(17) . ?
W2 O8 1.825(17) . ?
W2 O24 1.89(2) . ?
W2 O22 1.964(17) . ?
W2 O33 2.016(16) . ?
W2 O25 2.456(15) . ?
W3 O39 1.684(17) . ?
W3 O31 1.841(17) . ?
W3 O36 1.897(15) . ?
W3 O32 1.899(16) . ?
W3 O35 1.936(17) . ?
W3 O27 2.529(15) . ?
W4 O21 1.751(19) . ?
W4 O11 1.834(15) . ?
W4 O22 1.859(17) . ?
W4 O20 1.950(14) . ?
W4 O31 2.030(16) . ?
W4 O27 2.426(16) . ?
W5 O15 1.72(2) . ?
W5 O7 1.821(16) . ?
W5 O14 1.927(15) . ?
W5 O16 1.942(16) . ?
W5 O29 1.989(15) . ?
W5 O26 2.449(18) . ?
W6 O17 1.735(17) . ?
W6 O10 1.781(15) . ?
W6 O18 1.899(19) . ?
W6 O16 1.921(19) . ?
W6 O30 1.987(15) . ?
W6 O26 2.461(16) . ?
W7 O19 1.723(17) . ?
W7 O12 1.806(15) . ?
W7 O20 1.924(17) . ?
W7 O18 1.930(19) . ?
W7 O32 1.970(17) . ?
W7 O27 2.439(15) . ?
W8 O38 1.712(16) . ?
W8 O30 1.873(17) . ?
W8 O29 1.875(19) . ?
W8 O35 1.885(17) . ?
W8 O34 1.922(15) . ?
W8 O26 2.484(15) . ?
W9 O37 1.748(17) . ?
W9 O28 1.869(18) . ?
W9 O33 1.872(15) . ?
W9 O34 1.932(15) . ?
W9 O36 1.942(16) . ?
W9 O25 2.528(16) . ?
C1 N1 1.466(10) . ?
C1 C2 1.517(10) . ?
C2 N2 1.477(10) . ?
C3 N3 1.41(4) . ?
C3 C4 1.46(4) . ?
C4 N4 1.44(4) . ?
C5 C6 1.45(5) . ?
C5 N5 1.51(4) . ?
C6 N6 1.43(4) . ?
C7 C8 1.53(5) . ?
C7 N7 1.58(5) . ?
C8 N8 1.55(5) . ?
C9 O41 1.33(4) . ?
C9 O40 1.41(5) . ?
C9 C10 1.522(10) . ?
C11 O5 1.21(3) . ?
C11 O4 1.27(3) . ?
C11 C12 1.56(3) . ?
C13 O1 1.37(3) . ?
C13 C16 1.51(4) . ?
C14 O2 1.45(3) . ?
C14 C16 1.51(4) . ?
C15 O3 1.42(3) . ?
C15 C16 1.47(3) . ?
C16 N9 1.52(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 Ni1 O40 91.5(12) . . ?
N1 Ni1 O2 97.8(10) . . ?
O40 Ni1 O2 92.3(8) . . ?
N1 Ni1 N2 81.2(10) . . ?
O40 Ni1 N2 93.4(10) . . ?
O2 Ni1 N2 174.2(9) . . ?
N1 Ni1 O7 179.4(9) . . ?
O40 Ni1 O7 88.9(9) . . ?
O2 Ni1 O7 82.6(7) . . ?
N2 Ni1 O7 98.3(8) . . ?
N1 Ni1 O6 96.4(10) . . ?
O40 Ni1 O6 168.8(8) . . ?
O2 Ni1 O6 78.8(6) . . ?
N2 Ni1 O6 95.6(8) . . ?
O7 Ni1 O6 83.3(6) . . ?
O3 Ni2 O7 169.7(7) . . ?
O3 Ni2 O41 99.6(9) . . ?
O7 Ni2 O41 89.8(9) . . ?
O3 Ni2 O10 84.3(6) . . ?
O7 Ni2 O10 99.4(7) . . ?
O41 Ni2 O10 94.0(9) . . ?
O3 Ni2 O2 90.5(7) . . ?
O7 Ni2 O2 84.5(7) . . ?
O41 Ni2 O2 94.5(9) . . ?
O10 Ni2 O2 170.6(7) . . ?
O3 Ni2 O9 80.4(6) . . ?
O7 Ni2 O9 89.9(7) . . ?
O41 Ni2 O9 175.9(8) . . ?
O10 Ni2 O9 90.0(6) . . ?
O2 Ni2 O9 81.4(6) . . ?
O2 Ni3 O8 173.3(7) . . ?
O2 Ni3 O1 91.2(7) . . ?
O8 Ni3 O1 85.7(7) . . ?
O2 Ni3 O6 83.0(7) . . ?
O8 Ni3 O6 99.5(7) . . ?
O1 Ni3 O6 172.1(7) . . ?
O2 Ni3 O1W 97.4(8) . . ?
O8 Ni3 O1W 88.7(7) . . ?
O1 Ni3 O1W 94.1(7) . . ?
O6 Ni3 O1W 92.0(7) . . ?
O2 Ni3 O9 83.8(7) . . ?
O8 Ni3 O9 89.9(6) . . ?
O1 Ni3 O9 82.5(6) . . ?
O6 Ni3 O9 91.5(6) . . ?
O1W Ni3 O9 176.4(7) . . ?
N3 Ni4 O3 95.8(8) . . ?
N3 Ni4 O12 179.7(8) . . ?
O3 Ni4 O12 84.0(6) . . ?
N3 Ni4 N4 81.9(10) . . ?
O3 Ni4 N4 173.7(10) . . ?
O12 Ni4 N4 98.3(8) . . ?
N3 Ni4 O5 94.4(8) . . ?
O3 Ni4 O5 92.1(6) . . ?
O12 Ni4 O5 85.8(7) . . ?
N4 Ni4 O5 93.9(9) . . ?
N3 Ni4 O10 97.4(8) . . ?
O3 Ni4 O10 79.1(6) . . ?
O12 Ni4 O10 82.3(6) . . ?
N4 Ni4 O10 95.3(9) . . ?
O5 Ni4 O10 165.9(6) . . ?
O3 Ni5 O4 92.2(7) . . ?
O3 Ni5 O11 171.6(7) . . ?
O4 Ni5 O11 95.4(7) . . ?
O3 Ni5 O12 86.5(6) . . ?
O4 Ni5 O12 93.0(7) . . ?
O11 Ni5 O12 96.5(6) . . ?
O3 Ni5 O1 90.4(6) . . ?
O4 Ni5 O1 95.6(7) . . ?
O11 Ni5 O1 85.4(6) . . ?
O12 Ni5 O1 171.0(7) . . ?
O3 Ni5 O9 82.1(6) . . ?
O4 Ni5 O9 174.2(7) . . ?
O11 Ni5 O9 90.2(7) . . ?
O12 Ni5 O9 87.9(6) . . ?
O1 Ni5 O9 83.3(7) . . ?
N6 Ni6 O2W 94.4(8) . . ?
N6 Ni6 N5 83.2(9) . . ?
O2W Ni6 N5 91.0(9) . . ?
N6 Ni6 O11 179.1(9) . . ?
O2W Ni6 O11 86.4(7) . . ?
N5 Ni6 O11 97.3(7) . . ?
N6 Ni6 O1 97.4(8) . . ?
O2W Ni6 O1 90.1(7) . . ?
N5 Ni6 O1 178.8(9) . . ?
O11 Ni6 O1 82.1(6) . . ?
N6 Ni6 O8 94.4(8) . . ?
O2W Ni6 O8 167.3(7) . . ?
N5 Ni6 O8 99.1(9) . . ?
O11 Ni6 O8 84.8(7) . . ?
O1 Ni6 O8 79.8(7) . . ?
N7 Ni7 N7 180.0 . 3_556 ?
N7 Ni7 N8 84.1(13) . . ?
N7 Ni7 N8 95.9(13) 3_556 . ?
N7 Ni7 N8 95.9(13) . 3_556 ?
N7 Ni7 N8 84.1(13) 3_556 3_556 ?
N8 Ni7 N8 180.0 . 3_556 ?
N7 Ni7 O3W 93.5(12) . . ?
N7 Ni7 O3W 86.5(12) 3_556 . ?
N8 Ni7 O3W 89.7(14) . . ?
N8 Ni7 O3W 90.3(14) 3_556 . ?
N7 Ni7 O3W 86.5(12) . 3_556 ?
N7 Ni7 O3W 93.5(12) 3_556 3_556 ?
N8 Ni7 O3W 90.3(14) . 3_556 ?
N8 Ni7 O3W 89.7(14) 3_556 3_556 ?
O3W Ni7 O3W 180.0 . 3_556 ?
O27 P1 O26 110.5(9) . . ?
O27 P1 O25 109.7(9) . . ?
O26 P1 O25 107.7(9) . . ?
O27 P1 O9 109.4(9) . . ?
O26 P1 O9 110.8(9) . . ?
O25 P1 O9 108.8(8) . . ?
O13 W1 O6 103.7(7) . . ?
O13 W1 O14 101.3(8) . . ?
O6 W1 O14 92.0(8) . . ?
O13 W1 O28 100.1(8) . . ?
O6 W1 O28 156.1(7) . . ?
O14 W1 O28 86.1(7) . . ?
O13 W1 O24 102.2(8) . . ?
O6 W1 O24 89.2(7) . . ?
O14 W1 O24 155.5(8) . . ?
O28 W1 O24 83.1(7) . . ?
O13 W1 O25 170.6(7) . . ?
O6 W1 O25 84.1(6) . . ?
O14 W1 O25 83.5(7) . . ?
O28 W1 O25 72.0(6) . . ?
O24 W1 O25 72.2(6) . . ?
O23 W2 O8 104.0(8) . . ?
O23 W2 O24 101.3(8) . . ?
O8 W2 O24 89.2(8) . . ?
O23 W2 O22 101.9(8) . . ?
O8 W2 O22 91.1(7) . . ?
O24 W2 O22 156.1(7) . . ?
O23 W2 O33 99.8(7) . . ?
O8 W2 O33 156.0(7) . . ?
O24 W2 O33 84.3(7) . . ?
O22 W2 O33 85.8(7) . . ?
O23 W2 O25 170.5(8) . . ?
O8 W2 O25 83.3(6) . . ?
O24 W2 O25 72.6(6) . . ?
O22 W2 O25 83.7(6) . . ?
O33 W2 O25 72.7(6) . . ?
O39 W3 O31 100.2(8) . . ?
O39 W3 O36 102.6(8) . . ?
O31 W3 O36 89.2(7) . . ?
O39 W3 O32 101.2(8) . . ?
O31 W3 O32 88.3(7) . . ?
O36 W3 O32 156.2(7) . . ?
O39 W3 O35 104.3(8) . . ?
O31 W3 O35 155.5(7) . . ?
O36 W3 O35 84.2(7) . . ?
O32 W3 O35 88.3(7) . . ?
O39 W3 O27 170.6(8) . . ?
O31 W3 O27 73.0(6) . . ?
O36 W3 O27 84.1(6) . . ?
O32 W3 O27 72.5(6) . . ?
O35 W3 O27 82.8(6) . . ?
O21 W4 O11 103.5(8) . . ?
O21 W4 O22 101.1(8) . . ?
O11 W4 O22 92.5(7) . . ?
O21 W4 O20 101.9(9) . . ?
O11 W4 O20 90.2(7) . . ?
O22 W4 O20 155.6(7) . . ?
O21 W4 O31 100.9(8) . . ?
O11 W4 O31 155.5(7) . . ?
O22 W4 O31 84.8(7) . . ?
O20 W4 O31 82.7(6) . . ?
O21 W4 O27 172.5(7) . . ?
O11 W4 O27 82.9(6) . . ?
O22 W4 O27 82.3(6) . . ?
O20 W4 O27 73.9(6) . . ?
O31 W4 O27 72.6(6) . . ?
O15 W5 O7 105.3(9) . . ?
O15 W5 O14 101.3(9) . . ?
O7 W5 O14 89.6(7) . . ?
O15 W5 O16 101.9(9) . . ?
O7 W5 O16 89.5(7) . . ?
O14 W5 O16 156.2(8) . . ?
O15 W5 O29 100.8(9) . . ?
O7 W5 O29 153.9(8) . . ?
O14 W5 O29 86.0(7) . . ?
O16 W5 O29 84.5(7) . . ?
O15 W5 O26 170.8(7) . . ?
O7 W5 O26 82.1(7) . . ?
O14 W5 O26 83.9(7) . . ?
O16 W5 O26 72.4(7) . . ?
O29 W5 O26 71.9(7) . . ?
O17 W6 O10 104.3(8) . . ?
O17 W6 O18 100.8(8) . . ?
O10 W6 O18 92.7(7) . . ?
O17 W6 O16 102.3(8) . . ?
O10 W6 O16 89.4(7) . . ?
O18 W6 O16 155.4(7) . . ?
O17 W6 O30 99.5(7) . . ?
O10 W6 O30 156.1(7) . . ?
O18 W6 O30 84.7(8) . . ?
O16 W6 O30 83.5(7) . . ?
O17 W6 O26 170.1(7) . . ?
O10 W6 O26 84.3(6) . . ?
O18 W6 O26 83.4(7) . . ?
O16 W6 O26 72.4(6) . . ?
O30 W6 O26 71.8(6) . . ?
O19 W7 O12 104.7(8) . . ?
O19 W7 O20 99.2(8) . . ?
O12 W7 O20 90.8(7) . . ?
O19 W7 O18 101.4(8) . . ?
O12 W7 O18 88.9(8) . . ?
O20 W7 O18 158.7(7) . . ?
O19 W7 O32 101.0(8) . . ?
O12 W7 O32 154.1(7) . . ?
O20 W7 O32 82.5(7) . . ?
O18 W7 O32 88.5(7) . . ?
O19 W7 O27 171.7(8) . . ?
O12 W7 O27 80.5(6) . . ?
O20 W7 O27 74.0(6) . . ?
O18 W7 O27 84.9(6) . . ?
O32 W7 O27 73.6(6) . . ?
O38 W8 O30 101.4(7) . . ?
O38 W8 O29 100.9(8) . . ?
O30 W8 O29 90.3(8) . . ?
O38 W8 O35 102.2(8) . . ?
O30 W8 O35 90.1(7) . . ?
O29 W8 O35 156.3(7) . . ?
O38 W8 O34 101.0(7) . . ?
O30 W8 O34 157.6(7) . . ?
O29 W8 O34 85.8(8) . . ?
O35 W8 O34 84.9(7) . . ?
O38 W8 O26 171.3(7) . . ?
O30 W8 O26 73.0(6) . . ?
O29 W8 O26 72.8(7) . . ?
O35 W8 O26 84.7(6) . . ?
O34 W8 O26 84.8(6) . . ?
O37 W9 O28 103.0(8) . . ?
O37 W9 O33 101.2(8) . . ?
O28 W9 O33 89.6(7) . . ?
O37 W9 O34 102.2(8) . . ?
O28 W9 O34 88.6(7) . . ?
O33 W9 O34 156.3(7) . . ?
O37 W9 O36 101.6(8) . . ?
O28 W9 O36 155.4(7) . . ?
O33 W9 O36 86.2(7) . . ?
O34 W9 O36 85.7(7) . . ?
O37 W9 O25 171.3(7) . . ?
O28 W9 O25 70.9(6) . . ?
O33 W9 O25 73.1(6) . . ?
O34 W9 O25 84.0(6) . . ?
O36 W9 O25 84.7(6) . . ?
N1 C1 C2 111(3) . . ?
N2 C2 C1 109(2) . . ?
N3 C3 C4 109(3) . . ?
N4 C4 C3 113(3) . . ?
C6 C5 N5 109(3) . . ?
N6 C6 C5 111(3) . . ?
C8 C7 N7 104(4) . . ?
C7 C8 N8 107(3) . . ?
O41 C9 O40 137(3) . . ?
O41 C9 C10 116(3) . . ?
O40 C9 C10 107(3) . . ?
O5 C11 O4 131(2) . . ?
O5 C11 C12 115(2) . . ?
O4 C11 C12 113(2) . . ?
O1 C13 C16 117(2) . . ?
O2 C14 C16 114(2) . . ?
O3 C15 C16 115(2) . . ?
C15 C16 C13 117(2) . . ?
C15 C16 C14 111(2) . . ?
C13 C16 C14 110(2) . . ?
C15 C16 N9 105(2) . . ?
C13 C16 N9 111(2) . . ?
C14 C16 N9 102(2) . . ?
C1 N1 Ni1 107(2) . . ?
C2 N2 Ni1 112.4(17) . . ?
C3 N3 Ni4 111(2) . . ?
C4 N4 Ni4 107(2) . . ?
C5 N5 Ni6 107(2) . . ?
C6 N6 Ni6 107.7(18) . . ?
C7 N7 Ni7 110(2) . . ?
C8 N8 Ni7 108(2) . . ?
C13 O1 Ni3 116.4(18) . . ?
C13 O1 Ni5 116.4(15) . . ?
Ni3 O1 Ni5 100.6(7) . . ?
C13 O1 Ni6 125.5(18) . . ?
Ni3 O1 Ni6 98.1(7) . . ?
Ni5 O1 Ni6 95.1(7) . . ?
C14 O2 Ni3 116.8(16) . . ?
C14 O2 Ni1 123.1(16) . . ?
Ni3 O2 Ni1 101.7(7) . . ?
C14 O2 Ni2 114.4(14) . . ?
Ni3 O2 Ni2 102.1(8) . . ?
Ni1 O2 Ni2 94.9(7) . . ?
C15 O3 Ni2 113.6(14) . . ?
C15 O3 Ni5 118.9(14) . . ?
Ni2 O3 Ni5 104.0(7) . . ?
C15 O3 Ni4 121.4(13) . . ?
Ni2 O3 Ni4 102.1(6) . . ?
Ni5 O3 Ni4 93.4(6) . . ?
C11 O4 Ni5 122.5(15) . . ?
C11 O5 Ni4 124.5(16) . . ?
W1 O6 Ni3 132.8(9) . . ?
W1 O6 Ni1 127.1(9) . . ?
Ni3 O6 Ni1 95.8(7) . . ?
W5 O7 Ni2 135.0(10) . . ?
W5 O7 Ni1 128.7(9) . . ?
Ni2 O7 Ni1 95.0(7) . . ?
W2 O8 Ni3 134.1(9) . . ?
W2 O8 Ni6 126.6(10) . . ?
Ni3 O8 Ni6 95.6(7) . . ?
P1 O9 Ni5 124.4(10) . . ?
P1 O9 Ni3 123.1(9) . . ?
Ni5 O9 Ni3 93.6(6) . . ?
P1 O9 Ni2 121.3(9) . . ?
Ni5 O9 Ni2 93.4(6) . . ?
Ni3 O9 Ni2 92.6(6) . . ?
W6 O10 Ni2 133.4(9) . . ?
W6 O10 Ni4 128.1(8) . . ?
Ni2 O10 Ni4 93.8(6) . . ?
W4 O11 Ni5 135.1(9) . . ?
W4 O11 Ni6 125.9(8) . . ?
Ni5 O11 Ni6 95.9(6) . . ?
W7 O12 Ni5 137.6(9) . . ?
W7 O12 Ni4 130.1(9) . . ?
Ni5 O12 Ni4 91.7(6) . . ?
W1 O14 W5 148.4(11) . . ?
W6 O16 W5 126.0(9) . . ?
W6 O18 W7 148.2(9) . . ?
W7 O20 W4 123.0(9) . . ?
W4 O22 W2 149.0(10) . . ?
W2 O24 W1 125.5(8) . . ?
P1 O25 W1 128.3(9) . . ?
P1 O25 W2 124.6(9) . . ?
W1 O25 W2 89.6(5) . . ?
P1 O25 W9 125.5(8) . . ?
W1 O25 W9 88.6(5) . . ?
W2 O25 W9 88.0(5) . . ?
P1 O26 W5 126.8(9) . . ?
P1 O26 W6 125.3(9) . . ?
W5 O26 W6 89.0(6) . . ?
P1 O26 W8 126.5(9) . . ?
W5 O26 W8 88.7(5) . . ?
W6 O26 W8 88.4(5) . . ?
P1 O27 W4 127.6(8) . . ?
P1 O27 W7 125.2(8) . . ?
W4 O27 W7 88.8(5) . . ?
P1 O27 W3 126.6(8) . . ?
W4 O27 W3 88.2(5) . . ?
W7 O27 W3 87.8(5) . . ?
W9 O28 W1 128.3(9) . . ?
W8 O29 W5 126.2(10) . . ?
W8 O30 W6 126.6(8) . . ?
W3 O31 W4 126.0(9) . . ?
W3 O32 W7 125.9(9) . . ?
W9 O33 W2 125.9(8) . . ?
W8 O34 W9 149.6(11) . . ?
W8 O35 W3 153.5(9) . . ?
W3 O36 W9 151.3(9) . . ?
C9 O40 Ni1 117.9(19) . . ?
C9 O41 Ni2 117(2) . . ?

_refine_diff_density_max         4.436
_refine_diff_density_min         -2.775
_refine_diff_density_rms         0.502

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 1868971'
loop_
_audit_author_name
_audit_author_address
'[Ni(en)2][Ni6(en)3(?3-OH)3(1,3-bdc)(H2O)2(B-?-PW9O34)"9H2O'
;BIT
China
;
_audit_update_record             
;
2018-09-21 deposited with the CCDC.	2019-03-11 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C18 H67 N10 Ni7 O53 P W9'
_chemical_formula_weight         3368.40

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           19
_space_group_name_H-M_alt        'P 21 21 21'
_space_group_name_Hall           'P 2ac 2ab'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'-x, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'

_cell_length_a                   13.3441(3)
_cell_length_b                   14.2773(3)
_cell_length_c                   36.0138(11)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     6861.3(3)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       ?
_exptl_crystal_colour            ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.261
_exptl_crystal_F_000             6184
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.180
_exptl_crystal_size_mid          0.140
_exptl_crystal_size_min          0.100
_exptl_absorpt_coefficient_mu    17.021
_shelx_estimated_absorpt_T_min   0.150
_shelx_estimated_absorpt_T_max   0.281
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            28423
_diffrn_reflns_av_unetI/netI     0.0647
_diffrn_reflns_av_R_equivalents  0.0475
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_l_min       -42
_diffrn_reflns_limit_l_max       42
_diffrn_reflns_theta_min         2.853
_diffrn_reflns_theta_max         25.006
_diffrn_reflns_theta_full        25.006
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_point_group_measured_fraction_full 0.993
_reflns_number_total             12000
_reflns_number_gt                11078
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.800
_reflns_Friedel_fraction_max     0.987
_reflns_Friedel_fraction_full    0.987

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0461P)²+162.9642P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   mixed
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Flack x determined using 4225 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.382(8)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         12000
_refine_ls_number_parameters     883
_refine_ls_number_restraints     171
_refine_ls_R_factor_all          0.0570
_refine_ls_R_factor_gt           0.0510
_refine_ls_wR_factor_ref         0.1137
_refine_ls_wR_factor_gt          0.1105
_refine_ls_goodness_of_fit_ref   1.042
_refine_ls_restrained_S_all      1.037
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 0.2052(2) 0.0669(2) 0.77178(10) 0.0206(7) Uani 1 1 d . . . . .
Ni2 Ni 0.4362(2) 0.1010(2) 0.77883(9) 0.0171(7) Uani 1 1 d . . . . .
Ni3 Ni 0.3115(2) -0.0091(2) 0.83823(9) 0.0171(7) Uani 1 1 d . . . . .
Ni4 Ni 0.6680(2) 0.1067(2) 0.78994(9) 0.0189(7) Uani 1 1 d . . . . .
Ni5 Ni 0.5460(2) 0.0064(2) 0.84643(9) 0.0179(7) Uani 1 1 d . . . . .
Ni6 Ni 0.4204(3) -0.1078(3) 0.90284(11) 0.0272(8) Uani 1 1 d . . . . .
Ni7 Ni 0.3844(3) 0.3401(4) 0.03626(12) 0.0471(12) Uani 1 1 d . . . . .
P1 P 0.4044(4) 0.1974(4) 0.86177(17) 0.0091(12) Uani 1 1 d . U . . .
W1 W 0.23553(8) 0.32108(8) 0.92293(3) 0.0217(2) Uani 1 1 d . . . . .
W2 W 0.13840(7) 0.18361(7) 0.85281(3) 0.0191(2) Uani 1 1 d . . . . .
W3 W 0.54429(8) 0.32486(7) 0.79604(3) 0.0182(2) Uani 1 1 d . . . . .
W4 W 0.52374(8) 0.09795(8) 0.93968(3) 0.0219(3) Uani 1 1 d . . . . .
W5 W 0.25054(9) 0.07870(9) 0.92703(4) 0.0212(3) Uani 1 1 d . U . . .
W6 W 0.66540(8) 0.21625(8) 0.87693(3) 0.0200(2) Uani 1 1 d . . . . .
W7 W 0.51060(8) 0.33966(8) 0.93553(3) 0.0235(3) Uani 1 1 d . . . . .
W8 W 0.29123(8) 0.30895(7) 0.78383(3) 0.0188(2) Uani 1 1 d . . . . .
W9 W 0.38689(9) 0.45022(7) 0.85366(3) 0.0221(3) Uani 1 1 d . . . . .
C1 C 0.071(2) 0.145(3) 0.7169(7) 0.068(13) Uani 1 1 d D . . . .
H1A H 0.047207 0.205432 0.708289 0.082 Uiso 1 1 calc R U . . .
H1B H 0.019582 0.098887 0.710977 0.082 Uiso 1 1 calc R U . . .
C2 C 0.166(3) 0.120(3) 0.6966(9) 0.073(13) Uani 1 1 d D . . . .
H2A H 0.150760 0.101151 0.671328 0.087 Uiso 1 1 calc R U . . .
H2B H 0.209945 0.174217 0.695503 0.087 Uiso 1 1 calc R U . . .
C3 C 0.791(2) 0.137(3) 0.7245(10) 0.063(8) Uani 1 1 d D U . . .
H3A H 0.788199 0.162857 0.699639 0.076 Uiso 1 1 calc R U . . .
H3B H 0.840302 0.086792 0.724392 0.076 Uiso 1 1 calc R U . . .
C4 C 0.826(3) 0.213(3) 0.7510(6) 0.057(10) Uani 1 1 d D . . . .
H4A H 0.898580 0.212253 0.751945 0.068 Uiso 1 1 calc R U . . .
H4B H 0.805034 0.273014 0.741457 0.068 Uiso 1 1 calc R U . . .
C5 C 0.354(3) -0.217(2) 0.9642(12) 0.074(12) Uani 1 1 d D U . . .
H5A H 0.323857 -0.222117 0.988669 0.088 Uiso 1 1 calc R U . . .
H5B H 0.405322 -0.265020 0.961903 0.088 Uiso 1 1 calc R U . . .
C6 C 0.275(3) -0.229(3) 0.9343(8) 0.095(18) Uani 1 1 d D . . . .
H6A H 0.244970 -0.290572 0.936015 0.113 Uiso 1 1 calc R U . . .
H6B H 0.222909 -0.182415 0.937378 0.113 Uiso 1 1 calc R U . . .
C7 C 0.433(3) 0.164(3) 0.0583(12) 0.069(9) Uani 1 1 d . U . . .
H7A H 0.415234 0.168373 0.084376 0.083 Uiso 1 1 calc R U . . .
H7B H 0.478808 0.111937 0.055102 0.083 Uiso 1 1 calc R U . . .
C8 C 0.336(3) 0.148(3) 0.0344(10) 0.059(11) Uani 1 1 d . . . . .
H8A H 0.353105 0.115934 0.011450 0.070 Uiso 1 1 calc R U . . .
H8B H 0.288457 0.109538 0.047948 0.070 Uiso 1 1 calc R U . . .
C9 C 0.340(5) 0.525(5) 0.022(2) 0.13(2) Uani 1 1 d . U . . .
H9A H 0.290921 0.572407 0.028752 0.159 Uiso 1 1 calc R U . . .
H9B H 0.361876 0.537620 -0.003159 0.159 Uiso 1 1 calc R U . . .
C10 C 0.428(4) 0.531(4) 0.0480(15) 0.086(14) Uani 1 1 d . U . . .
H10A H 0.475276 0.578754 0.039707 0.103 Uiso 1 1 calc R U . . .
H10B H 0.406682 0.546321 0.072999 0.103 Uiso 1 1 calc R U . . .
C11 C 0.751(2) -0.055(2) 0.8308(9) 0.032(7) Uani 1 1 d . . . . .
C12 C 1.1214(19) -0.095(2) 0.8177(9) 0.030(7) Uani 1 1 d . . . . .
C13 C 0.8475(19) -0.107(2) 0.8419(8) 0.029(7) Uani 1 1 d . . . . .
C14 C 0.846(2) -0.182(2) 0.8668(8) 0.033(7) Uani 1 1 d . U . . .
H14 H 0.786119 -0.202428 0.876771 0.040 Uiso 1 1 calc R U . . .
C15 C 0.938(2) -0.225(2) 0.8770(11) 0.052(10) Uani 1 1 d . . . . .
H15 H 0.938570 -0.272932 0.894615 0.062 Uiso 1 1 calc R U . . .
C16 C 1.024(2) -0.196(2) 0.8604(8) 0.031(7) Uani 1 1 d . . . . .
H16 H 1.084378 -0.225391 0.866537 0.038 Uiso 1 1 calc R U . . .
C17 C 1.0246(19) -0.1260(16) 0.8352(8) 0.020(6) Uani 1 1 d . . . . .
C18 C 0.9393(19) -0.0808(19) 0.8259(8) 0.026(6) Uani 1 1 d . . . . .
H18 H 0.941404 -0.032036 0.808828 0.031 Uiso 1 1 calc R U . . .
N1 N 0.0847(18) 0.1482(17) 0.7572(6) 0.033(6) Uani 1 1 d D . . . .
H1C H 0.029774 0.127209 0.768504 0.039 Uiso 1 1 calc R U . . .
H1D H 0.095023 0.207043 0.764369 0.039 Uiso 1 1 calc R U . . .
N2 N 0.2171(17) 0.0432(15) 0.7159(7) 0.029(6) Uani 1 1 d D . . . .
H2C H 0.281356 0.041037 0.709322 0.035 Uiso 1 1 calc R U . . .
H2D H 0.188765 -0.011278 0.710104 0.035 Uiso 1 1 calc R U . . .
N3 N 0.6931(19) 0.099(2) 0.7344(8) 0.047(6) Uani 1 1 d D U . . .
H3C H 0.689827 0.039120 0.727241 0.056 Uiso 1 1 calc R U . . .
H3D H 0.645562 0.130286 0.722427 0.056 Uiso 1 1 calc R U . . .
N4 N 0.7869(14) 0.2016(15) 0.7888(5) 0.022(5) Uani 1 1 d D . . . .
H4C H 0.766209 0.256942 0.797262 0.026 Uiso 1 1 calc R U . . .
H4D H 0.835665 0.181416 0.803666 0.026 Uiso 1 1 calc R U . . .
N5 N 0.397(2) -0.1235(19) 0.9585(9) 0.056(8) Uani 1 1 d D U . . .
H5C H 0.454482 -0.118103 0.970840 0.067 Uiso 1 1 calc R U . . .
H5D H 0.354858 -0.079804 0.966770 0.067 Uiso 1 1 calc R U . . .
N6 N 0.323(2) -0.2174(18) 0.8977(7) 0.046(7) Uani 1 1 d D . . . .
H6C H 0.277591 -0.205337 0.880404 0.055 Uiso 1 1 calc R U . . .
H6D H 0.356101 -0.269345 0.891440 0.055 Uiso 1 1 calc R U . . .
N7 N 0.477(3) 0.249(3) 0.0458(10) 0.071(9) Uani 1 1 d . U . . .
H7C H 0.511880 0.237246 0.025247 0.085 Uiso 1 1 calc R U . . .
H7D H 0.519489 0.269083 0.063033 0.085 Uiso 1 1 calc R U . . .
N8 N 0.2932(19) 0.241(2) 0.0265(8) 0.044(7) Uani 1 1 d . . . . .
H8C H 0.238557 0.248567 0.040325 0.053 Uiso 1 1 calc R U . . .
H8D H 0.274815 0.242915 0.002783 0.053 Uiso 1 1 calc R U . . .
N9 N 0.296(2) 0.438(3) 0.0236(10) 0.063(9) Uani 1 1 d . . . . .
H9C H 0.268958 0.425386 0.001538 0.075 Uiso 1 1 calc R U . . .
H9D H 0.246563 0.439561 0.040140 0.075 Uiso 1 1 calc R U . . .
N10 N 0.474(2) 0.438(3) 0.0467(9) 0.060(9) Uani 1 1 d . . . . .
H10C H 0.503435 0.426698 0.068540 0.072 Uiso 1 1 calc R U . . .
H10D H 0.522278 0.438154 0.029535 0.072 Uiso 1 1 calc R U . . .
O1 O 0.3008(14) 0.4269(12) 0.8132(5) 0.026(4) Uani 1 1 d . . . . .
O2 O 1.1151(14) -0.0479(13) 0.7868(6) 0.031(5) Uani 1 1 d . . . . .
O3 O 0.4338(12) -0.0880(11) 0.8473(5) 0.017(4) Uani 1 1 d . . . . .
H3E H 0.440974 -0.136663 0.833973 0.020 Uiso 1 1 d R U . . .
O4 O 0.4735(14) 0.4174(13) 0.8929(5) 0.026(4) Uani 1 1 d . . . . .
O5 O 0.2009(13) 0.0914(13) 0.8281(5) 0.024(4) Uani 1 1 d . . . . .
O6 O 0.5154(14) 0.0103(13) 0.9033(5) 0.026(4) Uani 1 1 d . . . . .
O7 O 0.3715(14) 0.3260(12) 0.9420(5) 0.027(4) Uani 1 1 d . . . . .
O8 O 0.2830(13) 0.4029(12) 0.8846(5) 0.020(4) Uani 1 1 d . U . . .
O9 O 0.6369(12) 0.1190(12) 0.8461(5) 0.021(4) Uani 1 1 d . . . . .
O10 O 0.5449(12) 0.2033(12) 0.7830(5) 0.022(4) Uani 1 1 d . . . . .
O11 O 0.1902(13) 0.2759(12) 0.8195(5) 0.023(4) Uani 1 1 d . . . . .
O12 O 0.3153(12) 0.1871(13) 0.7732(5) 0.024(4) Uani 1 1 d . . . . .
O13 O 0.1317(12) 0.2845(13) 0.8900(5) 0.023(4) Uani 1 1 d . . . . .
O14 O 0.3849(13) 0.0998(13) 0.9464(5) 0.025(4) Uani 1 1 d . . . . .
O15 O 0.6207(14) 0.3034(12) 0.8396(5) 0.025(4) Uani 1 1 d . . . . .
O16 O 0.4977(15) 0.4415(12) 0.8204(6) 0.029(5) Uani 1 1 d . . . . .
O17 O 0.3334(12) 0.0033(11) 0.7844(5) 0.015(3) Uani 1 1 d . U . . .
H17A H 0.344758 -0.047565 0.772867 0.018 Uiso 1 1 d R U . . .
O18 O 0.4084(11) 0.2811(11) 0.8349(4) 0.011(3) Uani 1 1 d . . . . .
O19 O 0.6361(12) 0.3196(12) 0.9124(5) 0.021(4) Uani 1 1 d . . . . .
O20 O 0.3036(12) 0.1950(11) 0.8822(5) 0.018(4) Uani 1 1 d . . . . .
O21 O 0.4184(12) 0.1058(11) 0.8394(5) 0.016(4) Uani 1 1 d . U . . .
O22 O 0.1741(15) 0.3932(16) 0.9523(5) 0.035(5) Uani 1 1 d . . . . .
O23 O 0.2189(14) 0.2080(13) 0.9481(5) 0.027(4) Uani 1 1 d . U . . .
O24 O 0.5515(12) 0.0175(11) 0.7905(5) 0.017(4) Uani 1 1 d . U . . .
H24A H 0.557042 -0.032859 0.778057 0.020 Uiso 1 1 d R U . . .
O25 O 0.6340(13) 0.3720(12) 0.7672(5) 0.023(4) Uani 1 1 d . U . . .
O26 O 0.2998(13) -0.0065(11) 0.8947(5) 0.018(4) Uani 1 1 d . . . . .
O27 O 0.3751(15) 0.5687(14) 0.8588(6) 0.034(5) Uani 1 1 d . . . . .
O28 O 0.7624(14) 0.0054(13) 0.8065(5) 0.025(4) Uani 1 1 d . U . . .
O29 O 1.2013(13) -0.1071(12) 0.8349(5) 0.022(4) Uani 1 1 d . . . . .
O30 O 0.4888(12) 0.2078(12) 0.8909(5) 0.021(4) Uani 1 1 d . . . . .
O31 O 0.6720(13) -0.0765(13) 0.8487(6) 0.032(5) Uani 1 1 d . . . . .
O32 O 0.2181(16) 0.3465(15) 0.7482(5) 0.036(5) Uani 1 1 d . . . . .
O33 O 0.4242(12) 0.3440(12) 0.7660(5) 0.020(4) Uani 1 1 d . . . . .
O34 O 0.6534(12) 0.1376(13) 0.9194(5) 0.026(4) Uani 1 1 d . . . . .
O35 O 0.2006(14) 0.0114(15) 0.9612(5) 0.034(5) Uani 1 1 d . . . . .
O36 O 0.5419(16) 0.4195(15) 0.9683(6) 0.040(5) Uani 1 1 d . . . . .
O37 O 0.1366(13) 0.1024(12) 0.8968(5) 0.021(4) Uani 1 1 d . U . . .
O38 O 0.0172(12) 0.1778(12) 0.8380(5) 0.026(4) Uani 1 1 d . . . . .
O39 O 0.5608(15) 0.0364(14) 0.9780(6) 0.033(5) Uani 1 1 d . . . . .
O40 O 0.252(3) 0.114(3) 0.9299(13) 0.085(10) Uani 1 1 d . U . . .
O41 O 0.5257(13) 0.2278(14) 0.9623(5) 0.028(5) Uani 1 1 d . . . . .
O43 O 0.7905(15) 0.2277(14) 0.8743(5) 0.033(5) Uani 1 1 d . . . . .
O1W O 0.5528(18) -0.1869(18) 0.9044(7) 0.059(7) Uani 1 1 d . . . . .
O2W O 0.4503(14) 0.0943(13) 0.7215(5) 0.030(5) Uani 1 1 d . . . . .
O3W O 0.452(3) 0.2672(19) 0.6912(9) 0.087(11) Uani 1 1 d . . . . .
O4W O 0.151(3) 0.600(3) 0.8827(14) 0.132(16) Uani 1 1 d . . . . .
O5W O 0.513(4) 0.610(4) 0.9258(15) 0.163(19) Uani 1 1 d . U . . .
O6W O 0.622(3) 0.807(3) 0.9823(13) 0.134(15) Uani 1 1 d . U . . .
O7W O 0.025(3) 0.402(3) 0.7659(13) 0.137(15) Uani 1 1 d . U . . .
O8W O 0.075(4) 0.458(3) 0.8413(13) 0.136(16) Uani 1 1 d . U . . .
O9W O 0.118(4) 0.886(3) 0.6630(14) 0.152(18) Uani 1 1 d . U . . .
O10W O 0.566(3) 0.917(2) 0.0433(13) 0.128(15) Uani 1 1 d . . . . .
O11W O 0.166(3) 0.885(3) 0.0220(12) 0.121(14) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ni1 O17 1.989(16) . ?
Ni1 N2 2.05(3) . ?
Ni1 N1 2.05(2) . ?
Ni1 O5 2.058(18) . ?
Ni1 O2 2.104(19) 1_455 ?
Ni1 O12 2.260(17) . ?
Ni1 Ni3 2.986(5) . ?
Ni2 O17 1.967(16) . ?
Ni2 O24 1.992(16) . ?
Ni2 O12 2.039(18) . ?
Ni2 O10 2.064(17) . ?
Ni2 O2W 2.08(2) . ?
Ni2 O21 2.195(17) . ?
Ni3 O17 1.968(16) . ?
Ni3 O3 2.009(17) . ?
Ni3 O29 2.033(17) 1_455 ?
Ni3 O26 2.041(17) . ?
Ni3 O5 2.090(19) . ?
Ni3 O21 2.174(17) . ?
Ni4 O28 2.009(18) . ?
Ni4 O24 2.010(16) . ?
Ni4 N3 2.03(3) . ?
Ni4 O9 2.072(18) . ?
Ni4 N4 2.088(19) . ?
Ni4 O10 2.159(17) . ?
Ni4 Ni5 2.973(5) . ?
Ni5 O9 2.014(18) . ?
Ni5 O3 2.014(17) . ?
Ni5 O24 2.021(17) . ?
Ni5 O31 2.058(18) . ?
Ni5 O6 2.091(18) . ?
Ni5 O21 2.231(17) . ?
Ni6 O3 2.028(17) . ?
Ni6 N6 2.04(3) . ?
Ni6 N5 2.04(3) . ?
Ni6 O1W 2.10(2) . ?
Ni6 O6 2.11(2) . ?
Ni6 O26 2.184(18) . ?
Ni7 N7 1.83(3) . ?
Ni7 N10 1.88(3) . ?
Ni7 N9 1.89(3) . ?
Ni7 N8 1.90(3) . ?
P1 O20 1.533(17) . ?
P1 O18 1.539(16) . ?
P1 O30 1.547(17) . ?
P1 O21 1.548(17) . ?
W1 O22 1.69(2) . ?
W1 O23 1.864(19) . ?
W1 O13 1.898(18) . ?
W1 O8 1.917(17) . ?
W1 O7 1.942(19) . ?
W1 O20 2.495(17) . ?
W2 O38 1.705(17) . ?
W2 O5 1.795(18) . ?
W2 O11 1.912(18) . ?
W2 O37 1.962(18) . ?
W2 O13 1.968(18) . ?
W2 O20 2.450(17) . ?
W3 O25 1.722(18) . ?
W3 O10 1.798(17) . ?
W3 O15 1.897(18) . ?
W3 O33 1.952(17) . ?
W3 O16 1.983(19) . ?
W3 O18 2.374(16) . ?
W4 O39 1.709(19) . ?
W4 O6 1.814(18) . ?
W4 O14 1.869(18) . ?
W4 O34 1.962(16) . ?
W4 O41 2.03(2) . ?
W4 O30 2.401(16) . ?
W5 O35 1.698(19) . ?
W5 O26 1.807(16) . ?
W5 O37 1.901(17) . ?
W5 O14 1.946(17) . ?
W5 O23 2.040(19) . ?
W5 O20 2.422(16) . ?
W6 O43 1.68(2) . ?
W6 O9 1.818(18) . ?
W6 O34 1.903(19) . ?
W6 O15 1.925(18) . ?
W6 O19 1.990(17) . ?
W6 O30 2.413(17) . ?
W7 O36 1.69(2) . ?
W7 O41 1.88(2) . ?
W7 O7 1.881(19) . ?
W7 O19 1.893(17) . ?
W7 O4 1.958(18) . ?
W7 O30 2.491(18) . ?
W8 O32 1.699(19) . ?
W8 O12 1.810(18) . ?
W8 O11 1.921(18) . ?
W8 O33 1.952(17) . ?
W8 O1 1.993(19) . ?
W8 O18 2.446(15) . ?
W9 O27 1.71(2) . ?
W9 O4 1.885(19) . ?
W9 O1 1.88(2) . ?
W9 O8 1.901(17) . ?
W9 O16 1.91(2) . ?
W9 O18 2.523(16) . ?
C1 N1 1.465(14) . ?
C1 C2 1.513(14) . ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C2 N2 1.466(14) . ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 N3 1.466(14) . ?
C3 C4 1.511(14) . ?
C3 H3A 0.9700 . ?
C3 H3B 0.9700 . ?
C4 N4 1.466(13) . ?
C4 H4A 0.9700 . ?
C4 H4B 0.9700 . ?
C5 N5 1.471(14) . ?
C5 C6 1.516(14) . ?
C5 H5A 0.9700 . ?
C5 H5B 0.9700 . ?
C6 N6 1.472(14) . ?
C6 H6A 0.9700 . ?
C6 H6B 0.9700 . ?
C7 N7 1.42(5) . ?
C7 C8 1.56(5) . ?
C7 H7A 0.9700 . ?
C7 H7B 0.9700 . ?
C8 N8 1.47(5) . ?
C8 H8A 0.9700 . ?
C8 H8B 0.9700 . ?
C9 N9 1.38(7) . ?
C9 C10 1.51(8) . ?
C9 H9A 0.9700 . ?
C9 H9B 0.9700 . ?
C10 N10 1.47(6) . ?
C10 H10A 0.9700 . ?
C10 H10B 0.9700 . ?
C11 O28 1.24(3) . ?
C11 O31 1.28(3) . ?
C11 C13 1.53(4) . ?
C12 O29 1.25(3) . ?
C12 O2 1.30(4) . ?
C12 C17 1.51(4) . ?
C13 C14 1.39(4) . ?
C13 C18 1.40(4) . ?
C14 C15 1.42(4) . ?
C14 H14 0.9300 . ?
C15 C16 1.37(4) . ?
C15 H15 0.9300 . ?
C16 C17 1.35(4) . ?
C16 H16 0.9300 . ?
C17 C18 1.35(4) . ?
C18 H18 0.9300 . ?
N1 H1C 0.8900 . ?
N1 H1D 0.8900 . ?
N2 H2C 0.8900 . ?
N2 H2D 0.8900 . ?
N3 H3C 0.8900 . ?
N3 H3D 0.8900 . ?
N4 H4C 0.8900 . ?
N4 H4D 0.8900 . ?
N5 H5C 0.8900 . ?
N5 H5D 0.8900 . ?
N6 H6C 0.8900 . ?
N6 H6D 0.8900 . ?
N7 H7C 0.8900 . ?
N7 H7D 0.8900 . ?
N8 H8C 0.8900 . ?
N8 H8D 0.8900 . ?
N9 H9C 0.8900 . ?
N9 H9D 0.8900 . ?
N10 H10C 0.8900 . ?
N10 H10D 0.8900 . ?
O3 H3E 0.8502 . ?
O17 H17A 0.8501 . ?
O23 O40 1.55(4) . ?
O24 H24A 0.8502 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O17 Ni1 N2 94.7(7) . . ?
O17 Ni1 N1 172.3(9) . . ?
N2 Ni1 N1 84.4(8) . . ?
O17 Ni1 O5 82.9(7) . . ?
N2 Ni1 O5 177.1(8) . . ?
N1 Ni1 O5 97.7(8) . . ?
O17 Ni1 O2 94.4(7) . 1_455 ?
N2 Ni1 O2 99.6(9) . 1_455 ?
N1 Ni1 O2 93.3(9) . 1_455 ?
O5 Ni1 O2 82.2(8) . 1_455 ?
O17 Ni1 O12 77.5(7) . . ?
N2 Ni1 O12 95.6(8) . . ?
N1 Ni1 O12 94.9(9) . . ?
O5 Ni1 O12 82.4(7) . . ?
O2 Ni1 O12 163.3(8) 1_455 . ?
O17 Ni1 Ni3 40.7(5) . . ?
N2 Ni1 Ni3 133.7(6) . . ?
N1 Ni1 Ni3 141.5(7) . . ?
O5 Ni1 Ni3 44.4(5) . . ?
O2 Ni1 Ni3 77.5(6) 1_455 . ?
O12 Ni1 Ni3 87.1(5) . . ?
O17 Ni2 O24 95.3(7) . . ?
O17 Ni2 O12 83.5(7) . . ?
O24 Ni2 O12 173.5(7) . . ?
O17 Ni2 O10 169.9(7) . . ?
O24 Ni2 O10 82.3(7) . . ?
O12 Ni2 O10 97.8(7) . . ?
O17 Ni2 O2W 97.6(7) . . ?
O24 Ni2 O2W 96.5(7) . . ?
O12 Ni2 O2W 90.0(7) . . ?
O10 Ni2 O2W 92.4(7) . . ?
O17 Ni2 O21 81.1(7) . . ?
O24 Ni2 O21 83.8(7) . . ?
O12 Ni2 O21 89.7(7) . . ?
O10 Ni2 O21 88.9(7) . . ?
O2W Ni2 O21 178.7(7) . . ?
O17 Ni3 O3 95.2(7) . . ?
O17 Ni3 O29 96.3(7) . 1_455 ?
O3 Ni3 O29 102.2(7) . 1_455 ?
O17 Ni3 O26 172.6(7) . . ?
O3 Ni3 O26 84.9(7) . . ?
O29 Ni3 O26 90.9(7) 1_455 . ?
O17 Ni3 O5 82.6(7) . . ?
O3 Ni3 O5 170.5(7) . . ?
O29 Ni3 O5 87.2(7) 1_455 . ?
O26 Ni3 O5 96.2(7) . . ?
O17 Ni3 O21 81.6(7) . . ?
O3 Ni3 O21 83.5(6) . . ?
O29 Ni3 O21 174.1(7) 1_455 . ?
O26 Ni3 O21 91.0(7) . . ?
O5 Ni3 O21 87.1(7) . . ?
O17 Ni3 Ni1 41.3(5) . . ?
O3 Ni3 Ni1 136.0(5) . . ?
O29 Ni3 Ni1 81.9(5) 1_455 . ?
O26 Ni3 Ni1 139.1(5) . . ?
O5 Ni3 Ni1 43.5(5) . . ?
O21 Ni3 Ni1 93.0(4) . . ?
O28 Ni4 O24 91.5(7) . . ?
O28 Ni4 N3 98.5(10) . . ?
O24 Ni4 N3 95.9(9) . . ?
O28 Ni4 O9 84.1(7) . . ?
O24 Ni4 O9 83.6(7) . . ?
N3 Ni4 O9 177.4(10) . . ?
O28 Ni4 N4 89.8(8) . . ?
O24 Ni4 N4 178.7(8) . . ?
N3 Ni4 N4 83.8(9) . . ?
O9 Ni4 N4 96.7(7) . . ?
O28 Ni4 O10 166.2(7) . . ?
O24 Ni4 O10 79.5(6) . . ?
N3 Ni4 O10 92.7(10) . . ?
O9 Ni4 O10 84.6(7) . . ?
N4 Ni4 O10 99.3(7) . . ?
O28 Ni4 Ni5 78.1(5) . . ?
O24 Ni4 Ni5 42.6(5) . . ?
N3 Ni4 Ni5 137.5(8) . . ?
O9 Ni4 Ni5 42.5(5) . . ?
N4 Ni4 Ni5 137.9(6) . . ?
O10 Ni4 Ni5 88.3(5) . . ?
O9 Ni5 O3 169.0(7) . . ?
O9 Ni5 O24 84.8(7) . . ?
O3 Ni5 O24 95.5(7) . . ?
O9 Ni5 O31 88.1(8) . . ?
O3 Ni5 O31 102.8(7) . . ?
O24 Ni5 O31 93.1(8) . . ?
O9 Ni5 O6 95.9(7) . . ?
O3 Ni5 O6 81.8(7) . . ?
O24 Ni5 O6 169.1(7) . . ?
O31 Ni5 O6 97.8(8) . . ?
O9 Ni5 O21 87.2(6) . . ?
O3 Ni5 O21 82.0(6) . . ?
O24 Ni5 O21 82.2(6) . . ?
O31 Ni5 O21 173.7(7) . . ?
O6 Ni5 O21 86.9(7) . . ?
O9 Ni5 Ni4 44.1(5) . . ?
O3 Ni5 Ni4 137.7(5) . . ?
O24 Ni5 Ni4 42.3(5) . . ?
O31 Ni5 Ni4 81.8(6) . . ?
O6 Ni5 Ni4 139.9(6) . . ?
O21 Ni5 Ni4 91.9(4) . . ?
O3 Ni6 N6 94.3(9) . . ?
O3 Ni6 N5 175.9(10) . . ?
N6 Ni6 N5 84.7(11) . . ?
O3 Ni6 O1W 91.6(8) . . ?
N6 Ni6 O1W 97.2(12) . . ?
N5 Ni6 O1W 92.5(11) . . ?
O3 Ni6 O6 81.0(7) . . ?
N6 Ni6 O6 174.6(10) . . ?
N5 Ni6 O6 99.9(9) . . ?
O1W Ni6 O6 85.6(9) . . ?
O3 Ni6 O26 80.8(6) . . ?
N6 Ni6 O26 91.6(10) . . ?
N5 Ni6 O26 95.2(10) . . ?
O1W Ni6 O26 168.8(8) . . ?
O6 Ni6 O26 85.1(7) . . ?
N7 Ni7 N10 93.5(15) . . ?
N7 Ni7 N9 175.5(16) . . ?
N10 Ni7 N9 84.1(14) . . ?
N7 Ni7 N8 86.2(14) . . ?
N10 Ni7 N8 179.0(13) . . ?
N9 Ni7 N8 96.2(13) . . ?
O20 P1 O18 110.4(9) . . ?
O20 P1 O30 108.4(10) . . ?
O18 P1 O30 109.1(9) . . ?
O20 P1 O21 109.7(10) . . ?
O18 P1 O21 108.9(9) . . ?
O30 P1 O21 110.3(10) . . ?
O22 W1 O23 99.5(9) . . ?
O22 W1 O13 101.8(9) . . ?
O23 W1 O13 88.8(8) . . ?
O22 W1 O8 103.9(9) . . ?
O23 W1 O8 156.5(8) . . ?
O13 W1 O8 87.6(7) . . ?
O22 W1 O7 102.1(9) . . ?
O23 W1 O7 88.3(8) . . ?
O13 W1 O7 156.0(7) . . ?
O8 W1 O7 85.7(8) . . ?
O22 W1 O20 170.3(8) . . ?
O23 W1 O20 72.8(7) . . ?
O13 W1 O20 72.5(6) . . ?
O8 W1 O20 84.0(6) . . ?
O7 W1 O20 84.0(6) . . ?
O38 W2 O5 104.5(8) . . ?
O38 W2 O11 100.4(8) . . ?
O5 W2 O11 91.5(8) . . ?
O38 W2 O37 102.2(8) . . ?
O5 W2 O37 88.4(8) . . ?
O11 W2 O37 156.7(7) . . ?
O38 W2 O13 101.8(8) . . ?
O5 W2 O13 153.5(7) . . ?
O11 W2 O13 86.5(7) . . ?
O37 W2 O13 83.3(7) . . ?
O38 W2 O20 172.5(7) . . ?
O5 W2 O20 81.1(7) . . ?
O11 W2 O20 84.3(7) . . ?
O37 W2 O20 72.6(6) . . ?
O13 W2 O20 72.5(6) . . ?
O25 W3 O10 102.6(8) . . ?
O25 W3 O15 100.9(8) . . ?
O10 W3 O15 93.3(8) . . ?
O25 W3 O33 100.5(8) . . ?
O10 W3 O33 89.7(8) . . ?
O15 W3 O33 157.2(8) . . ?
O25 W3 O16 99.0(8) . . ?
O10 W3 O16 158.1(7) . . ?
O15 W3 O16 86.4(8) . . ?
O33 W3 O16 82.5(8) . . ?
O25 W3 O18 171.6(7) . . ?
O10 W3 O18 84.5(6) . . ?
O15 W3 O18 83.1(7) . . ?
O33 W3 O18 74.7(6) . . ?
O16 W3 O18 73.8(7) . . ?
O39 W4 O6 104.2(9) . . ?
O39 W4 O14 101.0(9) . . ?
O6 W4 O14 92.4(9) . . ?
O39 W4 O34 101.2(9) . . ?
O6 W4 O34 89.1(8) . . ?
O14 W4 O34 156.7(8) . . ?
O39 W4 O41 98.1(9) . . ?
O6 W4 O41 157.3(8) . . ?
O14 W4 O41 87.0(8) . . ?
O34 W4 O41 82.8(8) . . ?
O39 W4 O30 169.4(8) . . ?
O6 W4 O30 84.9(7) . . ?
O14 W4 O30 83.8(7) . . ?
O34 W4 O30 73.1(7) . . ?
O41 W4 O30 72.5(7) . . ?
O35 W5 O26 103.2(9) . . ?
O35 W5 O37 101.7(8) . . ?
O26 W5 O37 92.4(7) . . ?
O35 W5 O14 101.0(8) . . ?
O26 W5 O14 90.0(8) . . ?
O37 W5 O14 156.0(8) . . ?
O35 W5 O23 99.3(9) . . ?
O26 W5 O23 157.5(8) . . ?
O37 W5 O23 83.5(7) . . ?
O14 W5 O23 85.3(8) . . ?
O35 W5 O20 170.5(8) . . ?
O26 W5 O20 85.7(7) . . ?
O37 W5 O20 74.3(7) . . ?
O14 W5 O20 82.2(7) . . ?
O23 W5 O20 71.8(6) . . ?
O43 W6 O9 104.3(9) . . ?
O43 W6 O34 100.8(8) . . ?
O9 W6 O34 91.3(8) . . ?
O43 W6 O15 101.8(9) . . ?
O9 W6 O15 90.2(8) . . ?
O34 W6 O15 156.2(7) . . ?
O43 W6 O19 99.2(9) . . ?
O9 W6 O19 156.5(7) . . ?
O34 W6 O19 84.6(8) . . ?
O15 W6 O19 84.7(7) . . ?
O43 W6 O30 170.8(8) . . ?
O9 W6 O30 83.4(7) . . ?
O34 W6 O30 73.8(6) . . ?
O15 W6 O30 82.8(7) . . ?
O19 W6 O30 73.2(6) . . ?
O36 W7 O41 100.8(10) . . ?
O36 W7 O7 103.1(9) . . ?
O41 W7 O7 87.4(8) . . ?
O36 W7 O19 101.0(9) . . ?
O41 W7 O19 90.1(8) . . ?
O7 W7 O19 155.9(8) . . ?
O36 W7 O4 103.1(10) . . ?
O41 W7 O4 155.9(8) . . ?
O7 W7 O4 84.6(8) . . ?
O19 W7 O4 88.0(8) . . ?
O36 W7 O30 170.7(9) . . ?
O41 W7 O30 72.6(7) . . ?
O7 W7 O30 83.5(7) . . ?
O19 W7 O30 72.9(6) . . ?
O4 W7 O30 83.9(6) . . ?
O32 W8 O12 104.2(9) . . ?
O32 W8 O11 100.3(9) . . ?
O12 W8 O11 91.8(8) . . ?
O32 W8 O33 101.2(9) . . ?
O12 W8 O33 90.9(7) . . ?
O11 W8 O33 157.0(7) . . ?
O32 W8 O1 99.9(9) . . ?
O12 W8 O1 156.0(8) . . ?
O11 W8 O1 84.1(8) . . ?
O33 W8 O1 84.2(7) . . ?
O32 W8 O18 170.5(8) . . ?
O12 W8 O18 83.7(7) . . ?
O11 W8 O18 84.6(6) . . ?
O33 W8 O18 73.0(6) . . ?
O1 W8 O18 72.4(6) . . ?
O27 W9 O4 102.8(9) . . ?
O27 W9 O1 101.7(9) . . ?
O4 W9 O1 155.4(8) . . ?
O27 W9 O8 102.8(8) . . ?
O4 W9 O8 85.4(8) . . ?
O1 W9 O8 86.8(8) . . ?
O27 W9 O16 101.8(9) . . ?
O4 W9 O16 88.8(8) . . ?
O1 W9 O16 88.6(8) . . ?
O8 W9 O16 155.4(7) . . ?
O27 W9 O18 170.6(7) . . ?
O4 W9 O18 83.9(6) . . ?
O1 W9 O18 72.1(6) . . ?
O8 W9 O18 84.2(6) . . ?
O16 W9 O18 71.4(6) . . ?
N1 C1 C2 112(2) . . ?
N1 C1 H1A 109.1 . . ?
C2 C1 H1A 109.1 . . ?
N1 C1 H1B 109.1 . . ?
C2 C1 H1B 109.1 . . ?
H1A C1 H1B 107.9 . . ?
N2 C2 C1 110(3) . . ?
N2 C2 H2A 109.7 . . ?
C1 C2 H2A 109.7 . . ?
N2 C2 H2B 109.7 . . ?
C1 C2 H2B 109.7 . . ?
H2A C2 H2B 108.2 . . ?
N3 C3 C4 113(3) . . ?
N3 C3 H3A 109.0 . . ?
C4 C3 H3A 109.0 . . ?
N3 C3 H3B 109.0 . . ?
C4 C3 H3B 109.0 . . ?
H3A C3 H3B 107.8 . . ?
N4 C4 C3 114(3) . . ?
N4 C4 H4A 108.8 . . ?
C3 C4 H4A 108.8 . . ?
N4 C4 H4B 108.8 . . ?
C3 C4 H4B 108.8 . . ?
H4A C4 H4B 107.7 . . ?
N5 C5 C6 106(3) . . ?
N5 C5 H5A 110.6 . . ?
C6 C5 H5A 110.6 . . ?
N5 C5 H5B 110.6 . . ?
C6 C5 H5B 110.6 . . ?
H5A C5 H5B 108.7 . . ?
N6 C6 C5 109(3) . . ?
N6 C6 H6A 109.9 . . ?
C5 C6 H6A 109.9 . . ?
N6 C6 H6B 109.9 . . ?
C5 C6 H6B 109.9 . . ?
H6A C6 H6B 108.3 . . ?
N7 C7 C8 107(3) . . ?
N7 C7 H7A 110.3 . . ?
C8 C7 H7A 110.3 . . ?
N7 C7 H7B 110.3 . . ?
C8 C7 H7B 110.3 . . ?
H7A C7 H7B 108.6 . . ?
N8 C8 C7 107(3) . . ?
N8 C8 H8A 110.3 . . ?
C7 C8 H8A 110.3 . . ?
N8 C8 H8B 110.3 . . ?
C7 C8 H8B 110.3 . . ?
H8A C8 H8B 108.5 . . ?
N9 C9 C10 111(5) . . ?
N9 C9 H9A 109.4 . . ?
C10 C9 H9A 109.4 . . ?
N9 C9 H9B 109.4 . . ?
C10 C9 H9B 109.4 . . ?
H9A C9 H9B 108.0 . . ?
N10 C10 C9 105(5) . . ?
N10 C10 H10A 110.8 . . ?
C9 C10 H10A 110.8 . . ?
N10 C10 H10B 110.8 . . ?
C9 C10 H10B 110.8 . . ?
H10A C10 H10B 108.9 . . ?
O28 C11 O31 128(3) . . ?
O28 C11 C13 115(3) . . ?
O31 C11 C13 117(3) . . ?
O29 C12 O2 124(3) . . ?
O29 C12 C17 119(3) . . ?
O2 C12 C17 117(2) . . ?
C14 C13 C18 118(3) . . ?
C14 C13 C11 122(3) . . ?
C18 C13 C11 120(2) . . ?
C13 C14 C15 120(3) . . ?
C13 C14 H14 120.2 . . ?
C15 C14 H14 120.2 . . ?
C16 C15 C14 119(3) . . ?
C16 C15 H15 120.7 . . ?
C14 C15 H15 120.7 . . ?
C17 C16 C15 121(3) . . ?
C17 C16 H16 119.3 . . ?
C15 C16 H16 119.3 . . ?
C18 C17 C16 121(3) . . ?
C18 C17 C12 118(2) . . ?
C16 C17 C12 120(2) . . ?
C17 C18 C13 120(3) . . ?
C17 C18 H18 119.8 . . ?
C13 C18 H18 119.8 . . ?
C1 N1 Ni1 109.6(18) . . ?
C1 N1 H1C 109.8 . . ?
Ni1 N1 H1C 109.8 . . ?
C1 N1 H1D 109.8 . . ?
Ni1 N1 H1D 109.8 . . ?
H1C N1 H1D 108.2 . . ?
C2 N2 Ni1 107.9(19) . . ?
C2 N2 H2C 110.1 . . ?
Ni1 N2 H2C 110.1 . . ?
C2 N2 H2D 110.1 . . ?
Ni1 N2 H2D 110.1 . . ?
H2C N2 H2D 108.4 . . ?
C3 N3 Ni4 111(2) . . ?
C3 N3 H3C 109.3 . . ?
Ni4 N3 H3C 109.3 . . ?
C3 N3 H3D 109.3 . . ?
Ni4 N3 H3D 109.3 . . ?
H3C N3 H3D 108.0 . . ?
C4 N4 Ni4 110.9(17) . . ?
C4 N4 H4C 109.5 . . ?
Ni4 N4 H4C 109.5 . . ?
C4 N4 H4D 109.5 . . ?
Ni4 N4 H4D 109.5 . . ?
H4C N4 H4D 108.0 . . ?
C5 N5 Ni6 107(2) . . ?
C5 N5 H5C 110.3 . . ?
Ni6 N5 H5C 110.3 . . ?
C5 N5 H5D 110.3 . . ?
Ni6 N5 H5D 110.3 . . ?
H5C N5 H5D 108.5 . . ?
C6 N6 Ni6 106(2) . . ?
C6 N6 H6C 110.5 . . ?
Ni6 N6 H6C 110.5 . . ?
C6 N6 H6D 110.5 . . ?
Ni6 N6 H6D 110.5 . . ?
H6C N6 H6D 108.6 . . ?
C7 N7 Ni7 113(3) . . ?
C7 N7 H7C 109.0 . . ?
Ni7 N7 H7C 109.0 . . ?
C7 N7 H7D 109.0 . . ?
Ni7 N7 H7D 109.0 . . ?
H7C N7 H7D 107.8 . . ?
C8 N8 Ni7 113(2) . . ?
C8 N8 H8C 109.0 . . ?
Ni7 N8 H8C 109.0 . . ?
C8 N8 H8D 109.0 . . ?
Ni7 N8 H8D 109.0 . . ?
H8C N8 H8D 107.8 . . ?
C9 N9 Ni7 114(3) . . ?
C9 N9 H9C 108.6 . . ?
Ni7 N9 H9C 108.6 . . ?
C9 N9 H9D 108.6 . . ?
Ni7 N9 H9D 108.6 . . ?
H9C N9 H9D 107.6 . . ?
C10 N10 Ni7 114(3) . . ?
C10 N10 H10C 108.7 . . ?
Ni7 N10 H10C 108.7 . . ?
C10 N10 H10D 108.7 . . ?
Ni7 N10 H10D 108.7 . . ?
H10C N10 H10D 107.6 . . ?
W9 O1 W8 126.8(9) . . ?
C12 O2 Ni1 125.6(18) . 1_655 ?
Ni3 O3 Ni5 103.1(7) . . ?
Ni3 O3 Ni6 99.6(7) . . ?
Ni5 O3 Ni6 100.1(7) . . ?
Ni3 O3 H3E 117.3 . . ?
Ni5 O3 H3E 117.0 . . ?
Ni6 O3 H3E 116.9 . . ?
W9 O4 W7 152.1(11) . . ?
W2 O5 Ni1 128.8(10) . . ?
W2 O5 Ni3 138.1(10) . . ?
Ni1 O5 Ni3 92.1(7) . . ?
W4 O6 Ni5 135.5(10) . . ?
W4 O6 Ni6 126.5(9) . . ?
Ni5 O6 Ni6 95.0(8) . . ?
W7 O7 W1 151.9(11) . . ?
W9 O8 W1 151.5(10) . . ?
W6 O9 Ni5 137.1(9) . . ?
W6 O9 Ni4 128.2(9) . . ?
Ni5 O9 Ni4 93.4(7) . . ?
W3 O10 Ni2 134.4(9) . . ?
W3 O10 Ni4 126.2(9) . . ?
Ni2 O10 Ni4 95.2(7) . . ?
W2 O11 W8 147.4(10) . . ?
W8 O12 Ni2 134.4(9) . . ?
W8 O12 Ni1 128.2(9) . . ?
Ni2 O12 Ni1 93.3(7) . . ?
W1 O13 W2 126.4(9) . . ?
W4 O14 W5 149.9(12) . . ?
W3 O15 W6 148.0(10) . . ?
W9 O16 W3 125.1(9) . . ?
Ni2 O17 Ni3 105.5(8) . . ?
Ni2 O17 Ni1 104.6(7) . . ?
Ni3 O17 Ni1 98.0(7) . . ?
Ni2 O17 H17A 115.5 . . ?
Ni3 O17 H17A 115.6 . . ?
Ni1 O17 H17A 115.6 . . ?
P1 O18 W3 127.0(9) . . ?
P1 O18 W8 125.2(9) . . ?
W3 O18 W8 90.1(5) . . ?
P1 O18 W9 124.8(9) . . ?
W3 O18 W9 89.6(5) . . ?
W8 O18 W9 88.5(5) . . ?
W7 O19 W6 124.6(9) . . ?
P1 O20 W5 126.3(9) . . ?
P1 O20 W2 125.8(9) . . ?
W5 O20 W2 88.8(5) . . ?
P1 O20 W1 125.8(9) . . ?
W5 O20 W1 89.8(5) . . ?
W2 O20 W1 88.5(5) . . ?
P1 O21 Ni3 124.6(10) . . ?
P1 O21 Ni2 123.9(9) . . ?
Ni3 O21 Ni2 91.6(6) . . ?
P1 O21 Ni5 124.8(9) . . ?
Ni3 O21 Ni5 91.3(6) . . ?
Ni2 O21 Ni5 90.6(6) . . ?
O40 O23 W1 120.5(19) . . ?
O40 O23 W5 5.8(16) . . ?
W1 O23 W5 125.4(9) . . ?
Ni2 O24 Ni4 102.5(7) . . ?
Ni2 O24 Ni5 103.2(7) . . ?
Ni4 O24 Ni5 95.1(7) . . ?
Ni2 O24 H24A 117.5 . . ?
Ni4 O24 H24A 117.6 . . ?
Ni5 O24 H24A 117.6 . . ?
W5 O26 Ni3 133.0(9) . . ?
W5 O26 Ni6 128.9(9) . . ?
Ni3 O26 Ni6 93.7(7) . . ?
C11 O28 Ni4 129.6(19) . . ?
C12 O29 Ni3 123.4(19) . 1_655 ?
P1 O30 W4 125.1(10) . . ?
P1 O30 W6 125.0(9) . . ?
W4 O30 W6 89.7(5) . . ?
P1 O30 W7 126.6(9) . . ?
W4 O30 W7 90.0(6) . . ?
W6 O30 W7 89.0(6) . . ?
C11 O31 Ni5 121.3(19) . . ?
W3 O33 W8 121.9(9) . . ?
W6 O34 W4 123.0(9) . . ?
W5 O37 W2 123.9(9) . . ?
W7 O41 W4 124.8(9) . . ?

_refine_diff_density_max         2.179
_refine_diff_density_min         -1.780
_refine_diff_density_rms         0.304

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3_a
_database_code_depnum_ccdc_archive 'CCDC 1868913'
loop_
_audit_author_name
_audit_author_address
'[Ni(en)(H2O)4]3[Ni6(en)3(tris)(1,3-bdc)1.5(B-?-PW9O34)]2"3H2O'
;BIT
China
;
_audit_update_record             
;
2018-09-21 deposited with the CCDC.	2019-03-11 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C16.67 H32 N6.67 Ni5 O33.67 P0.67 W6'
_chemical_formula_weight         2281.78

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_H-M_alt        'R -3 :H'
_space_group_name_Hall           '-R 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'

_cell_length_a                   21.5089(16)
_cell_length_b                   21.5089(16)
_cell_length_c                   58.751(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     23539(4)
_cell_formula_units_Z            18
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?

_exptl_crystal_description       ?
_exptl_crystal_colour            ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.897
_exptl_crystal_F_000             18756
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.180
_exptl_crystal_size_min          0.160
_exptl_absorpt_coefficient_mu    15.000
_shelx_estimated_absorpt_T_min   0.153
_shelx_estimated_absorpt_T_max   0.198
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            74581
_diffrn_reflns_av_unetI/netI     0.0488
_diffrn_reflns_av_R_equivalents  0.0774
_diffrn_reflns_limit_h_min       -25
_diffrn_reflns_limit_h_max       25
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_k_max       25
_diffrn_reflns_limit_l_min       -69
_diffrn_reflns_limit_l_max       69
_diffrn_reflns_theta_min         1.040
_diffrn_reflns_theta_max         25.009
_diffrn_reflns_theta_full        25.009
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_point_group_measured_fraction_full 1.000
_reflns_number_total             9272
_reflns_number_gt                7287
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXT 2014/4 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.1061P)²+5053.5005P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    refU
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         9272
_refine_ls_number_parameters     623
_refine_ls_number_restraints     349
_refine_ls_R_factor_all          0.0941
_refine_ls_R_factor_gt           0.0712
_refine_ls_wR_factor_ref         0.2162
_refine_ls_wR_factor_gt          0.2003
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_restrained_S_all      1.026
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ni1 Ni 0.91708(11) 1.00209(11) 0.67462(4) 0.0197(5) Uani 1 1 d . . . . .
Ni2 Ni 0.83218(12) 0.84391(12) 0.67866(5) 0.0248(6) Uani 1 1 d . . . . .
Ni3 Ni 0.50150(12) 0.67830(12) 0.76053(4) 0.0218(5) Uani 1 1 d . . . . .
Ni4 Ni 0.33464(11) 0.58359(11) 0.76483(4) 0.0180(5) Uani 1 1 d . . . . .
Ni5 Ni 0.5927(2) 0.5804(3) 0.87244(7) 0.0819(15) Uani 1 1 d . . . . .
P1 P 1.000000 1.000000 0.62769(12) 0.0105(14) Uani 1 3 d S T P . .
P2 P 0.333333 0.666667 0.81161(11) 0.0066(13) Uani 1 3 d S T P . .
W1 W 0.52289(4) 0.76691(4) 0.81323(2) 0.0247(2) Uani 1 1 d . . . . .
W2 W 0.90579(4) 1.09697(4) 0.62736(2) 0.0272(2) Uani 1 1 d . . . . .
W3 W 0.42776(4) 0.56964(4) 0.81219(2) 0.0248(2) Uani 1 1 d . . . . .
W4 W 0.80987(4) 0.91354(4) 0.62642(2) 0.0278(2) Uani 1 1 d . . . . .
W5 W 0.33679(5) 0.56871(5) 0.86111(2) 0.0306(2) Uani 1 1 d . . . . .
W6 W 0.90296(5) 1.00545(5) 0.57853(2) 0.0432(3) Uani 1 1 d . . . . .
C1 C 0.7453(9) 0.7057(11) 0.7015(3) 0.047(5) Uani 1 1 d D U . . .
C2 C 0.7224(13) 0.6932(10) 0.6768(3) 0.045(5) Uani 1 1 d D U . . .
C3 C 0.6054(17) 0.6305(14) 0.7634(5) 0.068(6) Uani 1 1 d D U . . .
C4 C 0.5773(11) 0.6144(19) 0.7392(5) 0.078(7) Uani 1 1 d D U . . .
C5 C 0.7848(11) 0.9406(11) 0.7003(4) 0.032(3) Uani 1 1 d . U . . .
C6 C 0.7229(10) 0.9441(10) 0.7099(4) 0.027(3) Uani 1 1 d . U . . .
C7 C 0.6643(10) 0.8839(10) 0.7184(3) 0.027(3) Uani 1 1 d . U . . .
H7 H 0.663895 0.840465 0.718254 0.01(4) Uiso 1 1 calc R . . . .
C8 C 0.6057(10) 0.8861(10) 0.7273(4) 0.028(3) Uani 1 1 d . U . . .
C9 C 0.6045(10) 0.9488(10) 0.7271(3) 0.027(3) Uani 1 1 d . U . . .
H9 H 0.564222 0.949938 0.732323 0.00(4) Uiso 1 1 calc R . . . .
C10 C 0.6646(10) 1.0121(11) 0.7190(4) 0.029(3) Uani 1 1 d . U . . .
H10 H 0.664822 1.055419 0.719224 0.08(10) Uiso 1 1 calc R . . . .
C11 C 0.7233(11) 1.0089(11) 0.7108(4) 0.030(3) Uani 1 1 d . U . . .
H11 H 0.763439 1.050713 0.705737 0.07(9) Uiso 1 1 calc R . . . .
C12 C 0.5462(10) 0.8200(10) 0.7382(4) 0.027(3) Uani 1 1 d . U . . .
C13 C 0.459(2) 0.4414(17) 0.8820(5) 0.089(8) Uani 1 1 d D U . . .
C14 C 0.4688(15) 0.4862(18) 0.9031(6) 0.084(8) Uani 1 1 d D U . . .
C15 C 0.9332(11) 0.9314(10) 0.7156(5) 0.0568(13) Uani 1 1 d D U . . .
C16 C 1.000000 1.000000 0.7232(6) 0.0568(11) Uani 1 3 d DS TU P . .
C17 C 0.2645(15) 0.6014(16) 0.7245(7) 0.0954(13) Uani 1 1 d D U . . .
C18 C 0.333333 0.666667 0.7163(8) 0.0954(12) Uani 1 3 d DS TU P . .
N1 N 0.8204(8) 0.7647(8) 0.7012(3) 0.037(4) Uani 1 1 d D . . . .
N2 N 0.7375(10) 0.7608(9) 0.6658(3) 0.042(5) Uani 1 1 d D U . . .
N3 N 0.5969(10) 0.6889(10) 0.7730(4) 0.048(5) Uani 1 1 d D . . . .
N4 N 0.5033(10) 0.6018(10) 0.7395(3) 0.038(4) Uani 1 1 d D . . . .
N5 N 0.492(2) 0.4915(19) 0.8628(6) 0.109(10) Uani 1 1 d D U . . .
N6 N 0.5466(15) 0.5376(16) 0.9044(6) 0.090(9) Uani 1 1 d D U . . .
N7 N 1.000000 1.000000 0.7482(6) 0.0570(13) Uani 1 3 d DS TU P . .
N8 N 0.333333 0.666667 0.6913(8) 0.0954(13) Uani 1 3 d DS TU P . .
O1 O 0.8430(6) 0.9222(6) 0.6555(2) 0.023(3) Uani 1 1 d . . . . .
O2 O 0.9287(6) 1.0900(6) 0.6568(2) 0.024(3) Uani 1 1 d . . . . .
O3 O 0.8766(7) 1.1574(7) 0.6287(3) 0.036(4) Uani 1 1 d . . . . .
O4 O 0.8185(7) 1.0071(7) 0.6291(3) 0.031(3) Uani 1 1 d . . . . .
O5 O 0.8931(8) 1.0767(8) 0.5941(2) 0.038(4) Uani 1 1 d . . . . .
O6 O 0.8188(8) 0.9334(8) 0.5938(3) 0.038(4) Uani 1 1 d . . . . .
O7 O 0.9972(7) 0.9307(6) 0.6187(2) 0.025(3) Uani 1 1 d . . . . .
O8 O 1.000000 1.000000 0.6541(3) 0.018(4) Uani 1 3 d S T P . .
O9 O 1.0025(9) 1.0695(9) 0.5753(3) 0.044(4) Uani 1 1 d . U . . .
O10 O 0.8737(11) 1.0079(11) 0.5518(4) 0.067(5) Uani 1 1 d . U . . .
O11 O 0.8410(7) 0.8460(7) 0.6199(3) 0.031(3) Uani 1 1 d . . . . .
O12 O 0.7181(7) 0.8573(7) 0.6292(3) 0.037(4) Uani 1 1 d . . . . .
O13 O 0.9230(7) 0.9234(7) 0.6922(2) 0.022(3) Uani 1 1 d . U . . .
O14 O 0.7757(8) 0.8770(7) 0.6988(3) 0.047(5) Uani 1 1 d . . . . .
O15 O 0.8386(7) 0.9969(6) 0.6945(2) 0.028(3) Uani 1 1 d . . . . .
O16 O 0.4933(7) 0.8243(7) 0.7447(3) 0.029(3) Uani 1 1 d . . . . .
O17 O 0.5568(7) 0.7675(7) 0.7402(3) 0.032(3) Uani 1 1 d . . . . .
O18 O 0.4910(6) 0.7450(6) 0.7838(2) 0.020(3) Uani 1 1 d . U . . .
O19 O 0.6136(7) 0.8003(8) 0.8114(2) 0.032(3) Uani 1 1 d . . . . .
O20 O 0.5139(7) 0.7798(7) 0.8456(2) 0.023(3) Uani 1 1 d . U . . .
O21 O 0.4913(7) 0.6694(7) 0.8200(3) 0.031(3) Uani 1 1 d . . . . .
O22 O 0.4212(6) 0.5931(6) 0.7828(2) 0.018(3) Uani 1 1 d . . . . .
O23 O 0.3362(7) 0.6003(6) 0.8203(2) 0.025(3) Uani 1 1 d . . . . .
O24 O 0.333333 0.666667 0.7858(3) 0.015(4) Uani 1 3 d S T P . .
O25 O 0.4085(7) 0.5581(7) 0.8456(2) 0.028(3) Uani 1 1 d . U . . .
O26 O 0.4029(8) 0.6693(8) 0.8644(2) 0.033(3) Uani 1 1 d . U . . .
O27 O 0.3381(9) 0.5379(10) 0.8883(3) 0.049(4) Uani 1 1 d . . . . .
O28 O 0.2565(7) 0.5899(7) 0.7473(2) 0.022(3) Uani 1 1 d . U . . .
O29 O 0.3366(8) 0.4828(7) 0.8111(2) 0.028(3) Uani 1 1 d . . . . .
O30 O 0.4871(8) 0.5386(8) 0.8110(3) 0.036(4) Uani 1 1 d . . . . .
O1W O 0.5458(13) 0.6431(13) 0.8712(4) 0.085(7) Uani 1 1 d . U . . .
O2W O 0.6235(15) 0.5964(12) 0.8380(4) 0.088(7) Uani 1 1 d . . . . .
O3W O 0.6937(17) 0.6729(18) 0.8826(4) 0.112(10) Uani 1 1 d . . . . .
O4W O 0.650(2) 0.522(2) 0.8735(6) 0.138(12) Uani 1 1 d . U . . .
O5W O 0.6976(10) 0.7334(10) 0.8188(4) 0.066(6) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ni1 O13 1.997(13) 3_675 ?
Ni1 O1 2.004(13) . ?
Ni1 O15 2.009(13) . ?
Ni1 O13 2.040(12) . ?
Ni1 O2 2.065(13) . ?
Ni1 O8 2.172(12) . ?
Ni1 Ni2 2.959(3) . ?
Ni2 O13 2.007(13) . ?
Ni2 O14 2.060(15) . ?
Ni2 N2 2.07(2) . ?
Ni2 N1 2.069(18) . ?
Ni2 O1 2.085(13) . ?
Ni2 O2 2.158(13) 2_765 ?
Ni3 O28 2.011(13) 2_665 ?
Ni3 O17 2.060(14) . ?
Ni3 N4 2.073(17) . ?
Ni3 O18 2.075(12) . ?
Ni3 N3 2.081(19) . ?
Ni3 O22 2.210(12) . ?
Ni3 Ni4 2.954(3) 2_665 ?
Ni4 O28 1.998(13) 2_665 ?
Ni4 O16 2.001(13) 3_565 ?
Ni4 O18 2.012(13) 3_565 ?
Ni4 O28 2.034(13) . ?
Ni4 O22 2.059(12) . ?
Ni4 O24 2.183(11) . ?
Ni5 O1W 2.05(3) . ?
Ni5 O2W 2.11(3) . ?
Ni5 N6 2.11(3) . ?
Ni5 N5 2.12(4) . ?
Ni5 O3W 2.17(3) . ?
Ni5 O4W 2.17(4) . ?
P1 O8 1.55(2) . ?
P1 O7 1.554(12) . ?
P1 O7 1.554(12) 2_765 ?
P1 O7 1.554(12) 3_675 ?
P2 O24 1.52(2) . ?
P2 O23 1.545(12) 3_565 ?
P2 O23 1.545(13) 2_665 ?
P2 O23 1.546(12) . ?
W1 O19 1.713(13) . ?
W1 O18 1.830(12) . ?
W1 O21 1.895(14) . ?
W1 O29 1.938(15) 2_665 ?
W1 O20 1.948(13) . ?
W1 O23 2.423(12) 2_665 ?
W2 O3 1.704(14) . ?
W2 O2 1.822(14) . ?
W2 O4 1.909(13) . ?
W2 O11 1.918(13) 3_675 ?
W2 O5 1.989(15) . ?
W2 O7 2.433(12) 3_675 ?
W3 O30 1.712(14) . ?
W3 O22 1.826(12) . ?
W3 O29 1.917(14) . ?
W3 O21 1.938(13) . ?
W3 O25 1.997(14) . ?
W3 O23 2.417(13) . ?
W4 O12 1.731(13) . ?
W4 O1 1.825(13) . ?
W4 O11 1.917(14) . ?
W4 O4 1.933(13) . ?
W4 O6 1.954(15) . ?
W4 O7 2.421(12) 3_675 ?
W5 O27 1.734(15) . ?
W5 O20 1.898(13) 3_565 ?
W5 O25 1.900(14) . ?
W5 O26 1.905(14) 3_565 ?
W5 O26 1.914(15) . ?
W5 O23 2.495(14) . ?
W6 O10 1.70(2) . ?
W6 O5 1.886(16) . ?
W6 O9 1.888(17) . ?
W6 O6 1.916(16) . ?
W6 O9 1.934(16) 2_765 ?
W6 O7 2.458(14) 3_675 ?
C1 N1 1.473(10) . ?
C1 C2 1.514(10) . ?
C2 N2 1.473(10) . ?
C3 N3 1.470(10) . ?
C3 C4 1.518(10) . ?
C4 N4 1.474(10) . ?
C5 O15 1.23(2) . ?
C5 O14 1.29(2) . ?
C5 C6 1.48(3) . ?
C6 C7 1.37(3) . ?
C6 C11 1.39(3) . ?
C7 C8 1.39(3) . ?
C7 H7 0.9300 . ?
C8 C9 1.36(3) . ?
C8 C12 1.50(3) . ?
C9 C10 1.41(3) . ?
C9 H9 0.9300 . ?
C10 C11 1.38(3) . ?
C10 H10 0.9300 . ?
C11 H11 0.9300 . ?
C12 O16 1.25(2) . ?
C12 O17 1.26(2) . ?
C13 N5 1.471(10) . ?
C13 C14 1.521(10) . ?
C14 N6 1.476(10) . ?
C15 O13 1.39(3) . ?
C15 C16 1.522(10) . ?
C16 N7 1.471(10) . ?
C17 O28 1.36(4) . ?
C17 C18 1.521(10) . ?
C18 N8 1.471(10) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O13 Ni1 O1 171.9(5) 3_675 . ?
O13 Ni1 O15 97.7(6) 3_675 . ?
O1 Ni1 O15 89.6(5) . . ?
O13 Ni1 O13 90.3(7) 3_675 . ?
O1 Ni1 O13 85.7(5) . . ?
O15 Ni1 O13 93.4(5) . . ?
O13 Ni1 O2 82.8(5) 3_675 . ?
O1 Ni1 O2 100.4(5) . . ?
O15 Ni1 O2 93.4(5) . . ?
O13 Ni1 O2 170.9(5) . . ?
O13 Ni1 O8 83.6(5) 3_675 . ?
O1 Ni1 O8 88.9(5) . . ?
O15 Ni1 O8 175.8(4) . . ?
O13 Ni1 O8 82.6(5) . . ?
O2 Ni1 O8 90.7(5) . . ?
O13 Ni1 Ni2 132.5(4) 3_675 . ?
O1 Ni1 Ni2 44.7(4) . . ?
O15 Ni1 Ni2 82.6(4) . . ?
O13 Ni1 Ni2 42.6(4) . . ?
O2 Ni1 Ni2 144.7(4) . . ?
O8 Ni1 Ni2 93.54(9) . . ?
O13 Ni2 O14 88.2(6) . . ?
O13 Ni2 N2 178.1(7) . . ?
O14 Ni2 N2 90.7(7) . . ?
O13 Ni2 N1 96.6(6) . . ?
O14 Ni2 N1 93.8(7) . . ?
N2 Ni2 N1 81.9(7) . . ?
O13 Ni2 O1 84.4(5) . . ?
O14 Ni2 O1 86.7(6) . . ?
N2 Ni2 O1 97.1(6) . . ?
N1 Ni2 O1 178.9(7) . . ?
O13 Ni2 O2 80.2(5) . 2_765 ?
O14 Ni2 O2 165.2(5) . 2_765 ?
N2 Ni2 O2 101.0(7) . 2_765 ?
N1 Ni2 O2 96.8(6) . 2_765 ?
O1 Ni2 O2 82.9(5) . 2_765 ?
O13 Ni2 Ni1 43.5(4) . . ?
O14 Ni2 Ni1 77.3(4) . . ?
N2 Ni2 Ni1 137.7(5) . . ?
N1 Ni2 Ni1 138.5(5) . . ?
O1 Ni2 Ni1 42.6(4) . . ?
O2 Ni2 Ni1 87.9(3) 2_765 . ?
O28 Ni3 O17 88.0(5) 2_665 . ?
O28 Ni3 N4 94.3(6) 2_665 . ?
O17 Ni3 N4 99.4(7) . . ?
O28 Ni3 O18 84.6(5) 2_665 . ?
O17 Ni3 O18 87.2(5) . . ?
N4 Ni3 O18 173.3(7) . . ?
O28 Ni3 N3 177.7(7) 2_665 . ?
O17 Ni3 N3 91.4(8) . . ?
N4 Ni3 N3 83.6(7) . . ?
O18 Ni3 N3 97.7(6) . . ?
O28 Ni3 O22 79.4(5) 2_665 . ?
O17 Ni3 O22 164.5(5) . . ?
N4 Ni3 O22 90.6(6) . . ?
O18 Ni3 O22 82.7(5) . . ?
N3 Ni3 O22 101.6(7) . . ?
O28 Ni3 Ni4 43.4(4) 2_665 2_665 ?
O17 Ni3 Ni4 77.2(4) . 2_665 ?
N4 Ni3 Ni4 137.2(5) . 2_665 ?
O18 Ni3 Ni4 42.9(3) . 2_665 ?
N3 Ni3 Ni4 138.5(5) . 2_665 ?
O22 Ni3 Ni4 87.4(3) . 2_665 ?
O28 Ni4 O16 96.5(5) 2_665 3_565 ?
O28 Ni4 O18 172.3(5) 2_665 3_565 ?
O16 Ni4 O18 90.4(5) 3_565 3_565 ?
O28 Ni4 O28 90.4(7) 2_665 . ?
O16 Ni4 O28 93.6(5) 3_565 . ?
O18 Ni4 O28 85.6(5) 3_565 . ?
O28 Ni4 O22 83.4(5) 2_665 . ?
O16 Ni4 O22 92.5(5) 3_565 . ?
O18 Ni4 O22 99.9(5) 3_565 . ?
O28 Ni4 O22 171.7(5) . . ?
O28 Ni4 O24 84.1(5) 2_665 . ?
O16 Ni4 O24 176.8(5) 3_565 . ?
O18 Ni4 O24 88.9(5) 3_565 . ?
O28 Ni4 O24 83.3(5) . . ?
O22 Ni4 O24 90.6(4) . . ?
O28 Ni4 Ni3 132.7(4) 2_665 3_565 ?
O16 Ni4 Ni3 83.1(4) 3_565 3_565 ?
O18 Ni4 Ni3 44.6(4) 3_565 3_565 ?
O28 Ni4 Ni3 42.8(4) . 3_565 ?
O22 Ni4 Ni3 143.9(4) . 3_565 ?
O24 Ni4 Ni3 94.26(9) . 3_565 ?
O1W Ni5 O2W 94.4(10) . . ?
O1W Ni5 N6 92.3(11) . . ?
O2W Ni5 N6 165.8(11) . . ?
O1W Ni5 N5 88.3(13) . . ?
O2W Ni5 N5 89.3(12) . . ?
N6 Ni5 N5 78.4(12) . . ?
O1W Ni5 O3W 90.2(12) . . ?
O2W Ni5 O3W 91.4(10) . . ?
N6 Ni5 O3W 101.1(11) . . ?
N5 Ni5 O3W 178.3(14) . . ?
O1W Ni5 O4W 175.6(13) . . ?
O2W Ni5 O4W 84.2(12) . . ?
N6 Ni5 O4W 90.0(13) . . ?
N5 Ni5 O4W 95.9(15) . . ?
O3W Ni5 O4W 85.7(14) . . ?
O8 P1 O7 109.9(6) . . ?
O8 P1 O7 109.9(6) . 2_765 ?
O7 P1 O7 109.1(6) . 2_765 ?
O8 P1 O7 109.9(6) . 3_675 ?
O7 P1 O7 109.1(6) . 3_675 ?
O7 P1 O7 109.1(6) 2_765 3_675 ?
O24 P2 O23 109.2(6) . 3_565 ?
O24 P2 O23 109.2(6) . 2_665 ?
O23 P2 O23 109.7(6) 3_565 2_665 ?
O24 P2 O23 109.2(6) . . ?
O23 P2 O23 109.7(6) 3_565 . ?
O23 P2 O23 109.7(6) 2_665 . ?
O19 W1 O18 104.5(6) . . ?
O19 W1 O21 100.4(6) . . ?
O18 W1 O21 91.9(6) . . ?
O19 W1 O29 101.5(6) . 2_665 ?
O18 W1 O29 89.6(5) . 2_665 ?
O21 W1 O29 157.0(6) . 2_665 ?
O19 W1 O20 100.1(6) . . ?
O18 W1 O20 155.2(5) . . ?
O21 W1 O20 86.9(6) . . ?
O29 W1 O20 82.3(5) 2_665 . ?
O19 W1 O23 170.4(6) . 2_665 ?
O18 W1 O23 82.7(5) . 2_665 ?
O21 W1 O23 85.5(5) . 2_665 ?
O29 W1 O23 71.9(5) 2_665 2_665 ?
O20 W1 O23 72.5(5) . 2_665 ?
O3 W2 O2 103.7(7) . . ?
O3 W2 O4 102.6(6) . . ?
O2 W2 O4 92.0(6) . . ?
O3 W2 O11 100.7(6) . 3_675 ?
O2 W2 O11 91.2(6) . 3_675 ?
O4 W2 O11 155.0(6) . 3_675 ?
O3 W2 O5 98.6(7) . . ?
O2 W2 O5 157.7(6) . . ?
O4 W2 O5 82.8(7) . . ?
O11 W2 O5 84.9(7) 3_675 . ?
O3 W2 O7 168.8(6) . 3_675 ?
O2 W2 O7 86.6(5) . 3_675 ?
O4 W2 O7 72.3(5) . 3_675 ?
O11 W2 O7 83.1(5) 3_675 3_675 ?
O5 W2 O7 71.1(5) . 3_675 ?
O30 W3 O22 104.2(7) . . ?
O30 W3 O29 102.5(6) . . ?
O22 W3 O29 93.2(5) . . ?
O30 W3 O21 101.0(6) . . ?
O22 W3 O21 91.6(6) . . ?
O29 W3 O21 154.0(6) . . ?
O30 W3 O25 98.0(7) . . ?
O22 W3 O25 157.8(5) . . ?
O29 W3 O25 82.2(6) . . ?
O21 W3 O25 83.8(6) . . ?
O30 W3 O23 169.2(6) . . ?
O22 W3 O23 85.7(5) . . ?
O29 W3 O23 72.3(5) . . ?
O21 W3 O23 82.6(5) . . ?
O25 W3 O23 72.2(5) . . ?
O12 W4 O1 103.5(7) . . ?
O12 W4 O11 101.4(6) . . ?
O1 W4 O11 89.8(6) . . ?
O12 W4 O4 101.6(6) . . ?
O1 W4 O4 89.3(6) . . ?
O11 W4 O4 156.5(6) . . ?
O12 W4 O6 101.4(7) . . ?
O1 W4 O6 155.0(6) . . ?
O11 W4 O6 86.4(6) . . ?
O4 W4 O6 84.6(6) . . ?
O12 W4 O7 171.2(6) . 3_675 ?
O1 W4 O7 82.9(5) . 3_675 ?
O11 W4 O7 84.4(5) . 3_675 ?
O4 W4 O7 72.2(5) . 3_675 ?
O6 W4 O7 72.1(6) . 3_675 ?
O27 W5 O20 104.0(7) . 3_565 ?
O27 W5 O25 103.0(7) . . ?
O20 W5 O25 88.8(6) 3_565 . ?
O27 W5 O26 101.4(8) . 3_565 ?
O20 W5 O26 87.3(6) 3_565 3_565 ?
O25 W5 O26 155.5(6) . 3_565 ?
O27 W5 O26 101.2(8) . . ?
O20 W5 O26 154.4(6) 3_565 . ?
O25 W5 O26 89.7(6) . . ?
O26 W5 O26 83.5(9) 3_565 . ?
O27 W5 O23 173.0(7) . . ?
O20 W5 O23 71.6(5) 3_565 . ?
O25 W5 O23 71.8(5) . . ?
O26 W5 O23 84.1(5) 3_565 . ?
O26 W5 O23 83.7(5) . . ?
O10 W6 O5 103.3(8) . . ?
O10 W6 O9 100.7(9) . . ?
O5 W6 O9 90.2(7) . . ?
O10 W6 O6 104.0(8) . . ?
O5 W6 O6 89.2(7) . . ?
O9 W6 O6 154.8(7) . . ?
O10 W6 O9 101.6(9) . 2_765 ?
O5 W6 O9 155.1(7) . 2_765 ?
O9 W6 O9 83.4(10) . 2_765 ?
O6 W6 O9 86.6(7) . 2_765 ?
O10 W6 O7 173.5(8) . 3_675 ?
O5 W6 O7 72.0(5) . 3_675 ?
O9 W6 O7 84.0(6) . 3_675 ?
O6 W6 O7 71.8(5) . 3_675 ?
O9 W6 O7 83.3(6) 2_765 3_675 ?
N1 C1 C2 104.9(17) . . ?
N2 C2 C1 110.8(17) . . ?
N3 C3 C4 110(2) . . ?
N4 C4 C3 107(2) . . ?
O15 C5 O14 126.5(19) . . ?
O15 C5 C6 118.8(18) . . ?
O14 C5 C6 114.7(17) . . ?
C7 C6 C11 118.3(18) . . ?
C7 C6 C5 121.1(17) . . ?
C11 C6 C5 120.7(18) . . ?
C6 C7 C8 121.8(18) . . ?
C6 C7 H7 119.1 . . ?
C8 C7 H7 119.1 . . ?
C9 C8 C7 119.9(18) . . ?
C9 C8 C12 120.9(18) . . ?
C7 C8 C12 119.1(17) . . ?
C8 C9 C10 119.7(18) . . ?
C8 C9 H9 120.1 . . ?
C10 C9 H9 120.1 . . ?
C11 C10 C9 119.3(18) . . ?
C11 C10 H10 120.4 . . ?
C9 C10 H10 120.4 . . ?
C10 C11 C6 120.9(19) . . ?
C10 C11 H11 119.6 . . ?
C6 C11 H11 119.6 . . ?
O16 C12 O17 128.0(18) . . ?
O16 C12 C8 116.0(16) . . ?
O17 C12 C8 115.9(17) . . ?
N5 C13 C14 107(3) . . ?
N6 C14 C13 105(3) . . ?
O13 C15 C16 115(2) . . ?
N7 C16 C15 106.9(17) . . ?
N7 C16 C15 106.9(17) . 2_765 ?
C15 C16 C15 111.9(15) . 2_765 ?
N7 C16 C15 106.9(16) . 3_675 ?
C15 C16 C15 111.9(15) . 3_675 ?
C15 C16 C15 111.9(15) 2_765 3_675 ?
O28 C17 C18 117(4) . . ?
N8 C18 C17 108(2) . . ?
N8 C18 C17 108(2) . 3_565 ?
C17 C18 C17 111(2) . 3_565 ?
N8 C18 C17 108(2) . 2_665 ?
C17 C18 C17 111(2) . 2_665 ?
C17 C18 C17 111(2) 3_565 2_665 ?
C1 N1 Ni2 110.5(14) . . ?
C2 N2 Ni2 109.2(14) . . ?
C3 N3 Ni3 107.9(15) . . ?
C4 N4 Ni3 108.0(16) . . ?
C13 N5 Ni5 111(3) . . ?
C14 N6 Ni5 113(2) . . ?
W4 O1 Ni1 135.6(7) . . ?
W4 O1 Ni2 130.4(7) . . ?
Ni1 O1 Ni2 92.7(5) . . ?
W2 O2 Ni1 130.0(6) . . ?
W2 O2 Ni2 130.8(6) . 3_675 ?
Ni1 O2 Ni2 94.7(5) . 3_675 ?
W2 O4 W4 125.7(7) . . ?
W6 O5 W2 126.6(7) . . ?
W6 O6 W4 125.8(8) . . ?
P1 O7 W4 124.9(7) . 2_765 ?
P1 O7 W2 125.1(7) . 2_765 ?
W4 O7 W2 89.5(4) 2_765 2_765 ?
P1 O7 W6 126.1(8) . 2_765 ?
W4 O7 W6 89.9(4) 2_765 2_765 ?
W2 O7 W6 90.1(4) 2_765 2_765 ?
P1 O8 Ni1 123.7(5) . . ?
P1 O8 Ni1 123.7(5) . 3_675 ?
Ni1 O8 Ni1 92.2(6) . 3_675 ?
P1 O8 Ni1 123.7(5) . 2_765 ?
Ni1 O8 Ni1 92.2(6) . 2_765 ?
Ni1 O8 Ni1 92.2(6) 3_675 2_765 ?
W6 O9 W6 153.5(10) . 3_675 ?
W4 O11 W2 148.2(8) . 2_765 ?
C15 O13 Ni1 115.9(13) . 2_765 ?
C15 O13 Ni2 121.6(11) . . ?
Ni1 O13 Ni2 101.8(6) 2_765 . ?
C15 O13 Ni1 118.0(13) . . ?
Ni1 O13 Ni1 101.7(6) 2_765 . ?
Ni2 O13 Ni1 94.0(5) . . ?
C5 O14 Ni2 127.3(14) . . ?
C5 O15 Ni1 124.4(13) . . ?
C12 O16 Ni4 123.3(12) . 2_665 ?
C12 O17 Ni3 127.4(12) . . ?
W1 O18 Ni4 135.6(7) . 2_665 ?
W1 O18 Ni3 130.1(6) . . ?
Ni4 O18 Ni3 92.6(5) 2_665 . ?
W5 O20 W1 127.0(7) 2_665 . ?
W1 O21 W3 147.1(8) . . ?
W3 O22 Ni4 130.4(7) . . ?
W3 O22 Ni3 130.8(6) . . ?
Ni4 O22 Ni3 94.2(5) . . ?
P2 O23 W3 127.0(7) . . ?
P2 O23 W1 124.4(7) . 3_565 ?
W3 O23 W1 90.0(4) . 3_565 ?
P2 O23 W5 125.2(8) . . ?
W3 O23 W5 89.9(4) . . ?
W1 O23 W5 88.8(4) 3_565 . ?
P2 O24 Ni4 124.4(4) . . ?
P2 O24 Ni4 124.4(4) . 3_565 ?
Ni4 O24 Ni4 91.2(6) . 3_565 ?
P2 O24 Ni4 124.4(4) . 2_665 ?
Ni4 O24 Ni4 91.2(6) . 2_665 ?
Ni4 O24 Ni4 91.2(6) 3_565 2_665 ?
W5 O25 W3 125.9(7) . . ?
W5 O26 W5 153.3(8) 2_665 . ?
C17 O28 Ni4 114.6(19) . 3_565 ?
C17 O28 Ni3 122.0(14) . 3_565 ?
Ni4 O28 Ni3 102.6(6) 3_565 3_565 ?
C17 O28 Ni4 118.7(18) . . ?
Ni4 O28 Ni4 101.4(6) 3_565 . ?
Ni3 O28 Ni4 93.8(5) 3_565 . ?
W3 O29 W1 125.2(7) . 3_565 ?

_refine_diff_density_max         6.018
_refine_diff_density_min         -3.364
_refine_diff_density_rms         0.461

